A Review on Revolutionary Natural Biopolymer-Based Aerogels for Antibacterial Delivery Esam Bashir Yahya 1 , Fauziah Jummaat 2, *, A. A. Amirul 3, * , A. S. Adnan 2 , N. G. Olaiya 1 , C. K. Abdullah 1 , Samsul Rizal 4 , M. K. Mohamad Haafiz 1 and H. P. S. Abdul Khalil 1, * 1
2 3 4
School of Industrial Technology, Universiti Sains Malaysia, Penang 11800, Malaysia; [email protected]
(E.B.Y.); [email protected]
(N.G.O.); [email protected]
(C.K.A.); [email protected]
(M.K.M.H.) Management Science University Medical Centre, University Drive, Off Persiaran Olahraga, Section 13, Shah Alam, Selangor 40100, Malaysia; [email protected]
School of Biological Sciences, Universiti Sains Malaysia, Penang 11800, Malaysia Department of Mechanical Engineering, Universitas Syiah Kuala, Banda Aceh 23111, Indonesia; [email protected]
Correspondence: [email protected]
(F.J.); [email protected]
(A.A.A.); [email protected]
Received: 10 September 2020; Accepted: 27 September 2020; Published: 28 September 2020
Abstract: A biopolymer-based aerogel has been developed to become one of the most potentially utilized materials in different biomedical applications. The biopolymer-based aerogel has unique physical, chemical, and mechanical properties and these properties are used in tissue engineering, biosensing, diagnostic, medical implant and drug delivery applications. Biocompatible and non-toxic biopolymers such as chitosan, cellulose and alginates have been used to deliver antibiotics, plants extract, essential oils and metallic nanoparticles. Antibacterial aerogels have been used in superficial and chronic wound healing as dressing sheets. This review critically analyses the utilization of biopolymer-based aerogels in antibacterial delivery. The analysis shows the relationship between their properties and their applications in the wound healing process. Furthermore, highlights of the potentials, challenges and proposition of the application of biopolymer-based aerogels is explored. Keywords: nanocellulose; aerogel; biopolymer; antibacterial; drug delivery; wound healing
1. Introduction The aerogel is a novel material formed by replacing the liquid of a gel with gas without changing its structure. Aerogels were first prepared with a supercritical drying technique using alcohol as a liquid . A few years later, this material was further experimented and utilized in different applications. Abdul Khalil et al.  describe an aerogel as a material which contains more than 99% air and can be prepared from various precursor material. Often, aerogel is manufactured in multi-shape structures to serve different needs. The first aerogel was produced from silica gel as a precursor material . Aerogel has since been prepared from organic, inorganic, and even composites of different materials. At present, biopolymers have attracted a lot of research work for aerogel preparation with a focus in biomedical applications. Biomedical application of aerogel includes wound healing, tissue engineering scaffolds and drug delivery . Biopolymers have properties desirable for potential materials used in biomedical applications. These properties include biocompatibility, non-toxic, hemostasis and antibacterial properties. The antimicrobial properties of some biopolymers
Antibiotics 2020, 9, 648; doi:10.3390/antibiotics9100648
Antibiotics 2020, 9, 648 Antibiotics 2020, 9, x FOR PEER REVIEW
2 of 25 2 of 26
make desirable materials wound materials healing applications . Much research has conducted some them biopolymers make them in desirable in wound healing applications .been Much research on the preparation of biopolymer-based aerogels and its characterization. has been conducted on the preparation of biopolymer-based aerogels and its characterization. Furthermore, Furthermore, in vitro vitro and and in in vivo vivo analysis analysis have have been been conducted conducted to to evaluate evaluate its use in different different applications, applications, including antibacterial delivery. delivery. Even with the the considerable considerable developments developments in in aerogel aerogel preparation, its commercialization is still relatively slow. The number of companies producing preparation, its commercialization is still relatively slow. of companies producing aerogels proposed with a aerogels with withdesired desiredproperties propertiesfor fordifferent differentapplications applicationsisislow. low.Many Manyauthors authorshave have proposed with conviction that a lot a conviction that a lotofofnewer neweraerogels aerogelsare aregoing goingtotobebeprepared preparedininthe thenext nextfew fewyears. years. The The interest interest in in biopolymer-based biopolymer-based aerogels has grown, grown, as as indicated indicated by by the the number number of of publications publications each each year year as as Figure Figure 11 presents. presents.
Figure of scientific publications in the last ten years, contributing to the subjectto“biopolymers Figure 1.1.Number Number of scientific publications in the last ten years, contributing the subject aerogels” by year (Search conducted through Science Direct on 9 September 2020 (From 2009 to 2019)). “biopolymers aerogels” by year (Search conducted through Science Direct on 9 September 2020 (From
2009 to 2019)).
There are already several excellent review articles and books about the history, properties, medical andare non-medical applications aerogels [6–9]. and Also, the chemistry, physics,properties, synthesis, There already several excellentofreview articles books about the history, and theirand different applications have of been extensively discussed [2,10,11]. physics, However, not much medical non-medical applications aerogels [6–9]. Also, the chemistry, synthesis, and has been done explicitly regarding the utilization of biopolymer-based aerogels for antibacterial their different applications have been extensively discussed [2,10,11]. However, not much has been delivery. This review selectively examined biopolymer-based aerogels aerogels for used in antibacterial delivery. done explicitly regarding the utilization of biopolymer-based antibacterial delivery. This Biopolymer-based aerogels such as chitosan-based, cellulose-based and alginate-based aerogels were review selectively examined biopolymer-based aerogels used in antibacterial delivery. Biopolymerdiscussed extensively. review includes an overview of their properties and the most recent works based aerogels such asThis chitosan-based, cellulose-based and alginate-based aerogels were discussed utilizing these aerogels inincludes antibacterial delivery of applications. Additionally, the study further extensively. This review an overview their properties and the most recent worksdiscusses utilizing the role of biopolymer-based aerogels in superficial and deep wound healing and to stop hemorrhaging. these aerogels in antibacterial delivery applications. Additionally, the study further discusses the role The study also highlighted some of the challenges and propositions of these biopolymer-based aerogels of biopolymer-based aerogels in superficial and deep wound healing and to stop hemorrhaging. The in antibacterial deliverysome applications. study also highlighted of the challenges and propositions of these biopolymer-based aerogels
in antibacterial delivery applications. 2. Biopolymer-Based Aerogels Biopolymers defined as naturally occurring materials consist of repetitive monomeric units that 2. Biopolymer-Based Aerogels covalently bonded to form larger molecules, such as cellulose, collagen, and alginates, etc. In the past Biopolymers defined as naturally occurring materials consist of repetitive monomeric units that few years, biopolymers have been extensively used in aerogel preparation for different biomedical covalently bonded to form larger molecules, such as cellulose, collagen, and alginates, etc. In the past applications due to their unique properties . Aerogel was defined as a solid, ultra-lightweight and few years, biopolymers have been extensively used in aerogel preparation for different biomedical lucid open porous network, obtained from gel following the removal of the pore liquid without any applications due to their unique properties . Aerogel was defined as a solid, ultra-lightweight and significant modification in the network structure . Traditional materials for aerogel preparation lucid open porous network, obtained from gel following the removal of the pore liquid without any like silica, carbon, metals, and synthetic polymers present some drawbacks that limit their use in significant modification in the network structure . Traditional materials for aerogel preparation biomedical applications. These drawbacks include immunological rejection by the body and their high like silica, carbon, metals, and synthetic polymers present some drawbacks that limit their use in cytotoxicity, which may cause undesirable immunogenic response . The studies on biopolymers are biomedical applications. These drawbacks include immunological rejection by the body and their high cytotoxicity, which may cause undesirable immunogenic response . The studies on biopolymers are motivated by the search for sustainable precursors instead of using traditional oil-
Antibiotics 2020, 9, x FOR PEER REVIEW Antibiotics 2020, 9, x FOR PEER REVIEW Antibiotics 2020, 9, 9, x FOR Antibiotics 2020, 648 PEER REVIEW
3 of 26 3 of 26 3 of 26 25 3 of
based or or synthetic synthetic materials materials . . Furthermore, Furthermore, the the biopolymers biopolymers are are desired desired in in medical medical and and based biomedical applications due to their biocompatibility and non-cytotoxicity. based or synthetic materials . Furthermore, the biopolymers are desired in medical and biomedical applications due to their biocompatibility and non-cytotoxicity. motivated byaerogel the search fortosustainable precursors of using traditional oil-based or He synthetic The first first fabrication approach was used usedinstead by Kistler, Kistler, the father father of aerogels aerogels . used biomedical applications due their biocompatibility and non-cytotoxicity. The aerogel fabrication approach was by the of . He used materials . Furthermore, the biopolymers are desired in medical and biomedical applications due sodium silicate as precursor precursor material and was heated in an an autoclave above the critical. temperature The silicate first aerogel fabrication approach used by Kistler, the father ofthe aerogels He used sodium as material and heated itit in autoclave above critical temperature to their biocompatibility andmaterial non-cytotoxicity. with thesilicate presence of pressure. This approach approach later became became widely known as supercritical supercritical drying . . sodium as of precursor and heated it in an widely autoclave above the critical temperature with the presence pressure. This later known as drying The first aerogel fabrication approach was used by Kistler, the father of aerogels . He used A few few years later,of sol-gel approach was designed designed by Teichner Teichner and Nicoloan, where they they developed with the presence pressure. This approach later became widely known as supercritical drying . A years later, aa sol-gel approach was by and Nicoloan, where developed sodium silicate as precursor material and heated it in an autoclave above the critical temperature Kistler’s approach by using using tetramethyl orthosilicate (TMOS), and which was easier easier to remove remove than the the A few years later, a by sol-gel approach was orthosilicate designed by Teichner Nicoloan, where they developed Kistler’s approach tetramethyl (TMOS), which was to than with the presence of pressure. This approach later became widely known as supercritical drying . water glass that Kistler used during supercritical drying . Other methods have been used to Kistler’s approach by using tetramethyl orthosilicatedrying (TMOS), easier to remove water glass that Kistler used during supercritical .which Otherwas methods have beenthan usedthe to A few years later, a sol-gel approach was designed by Teichner and Nicoloan, where they developed fabricate biopolymer-based aerogels including freeze-drying , gas foaming foaming , , electrospinning water glass that Kistler used duringincluding supercritical drying ., Other methods haveelectrospinning been used to fabricate biopolymer-based aerogels freeze-drying gas Kistler’s approach by using tetramethyl orthosilicate (TMOS), which was easier todiscussed remove than , and thermal-induced phase separation , which all have been presented and by fabricate biopolymer-based aerogels including freeze-drying , gas foaming , electrospinning , and thermal-induced phase separation , which all have been presented and discussed by the water glass that Kistler used during supercritical drying . Other methods have been used Abdul Khalil et al. . Recently, a new generation of computer aid fabrication approaches have been , and thermal-induced phaseaseparation , which all have presented and discussed byto Abdul Khalil et al. . Recently, new generation of computer aidbeen fabrication approaches have been fabricate biopolymer-based aerogels including freeze-drying , gas foaming , electrospinning , developed, which areRecently, called rapid rapid prototyping . Variousaid computer-aided methods have havebeen been Abdul Khalilwhich et al. . a new generation. of computer fabrication approaches developed, are called prototyping Various computer-aided methods have been and thermal-induced phase separation which all haveusing been presented and by been Abdul fabricated to design design the desired shape, of 3D 3D. aerogels biopolymers asdiscussed bio-injected ink. developed, which are the called rapid prototyping Various computer-aided methods have fabricated to desired shape of aerogels using biopolymers as bio-injected ink. Khalil et al. . Recently, a new generation of computer aid fabrication approaches have been developed, Stereolithography , selective laser sintering , fused deposition deposition modelling , , and 3D 3D printing printing fabricated to design the desired shape of 3D aerogels using biopolymers as bio-injected ink. Stereolithography , selective laser sintering , fused modelling and whichare areexamples called , rapid prototyping . Various computer-aided methods have been fabricated to [24,25] of the most used fabrication techniques of biopolymer-based aerogels. Chitosan, Stereolithography selective laser sintering , fused deposition modelling , and 3D printing [24,25] are examples of the most used fabrication techniques of biopolymer-based aerogels. Chitosan, design the desired shape ofbeen 3D aerogels biopolymers asbiopolymer-based bio-injected Stereolithography , cellulose and alginate have used in using various medical applications applications dueink. to their their uniqueChitosan, biological [24,25] are examples of have the most fabrication techniques of aerogels. cellulose and alginate beenused used in various medical due to unique biological selective laser sintering , fused deposition modelling , and 3D printing [24,25] are examples characteristics such as ashave hemostatic properties, antibacterial and mucoadhesive mucoadhesive properties which are areof cellulose and alginate been used in various medical applications due to their unique biological characteristics such hemostatic properties, antibacterial and properties which the most usedsuch fabrication techniques ofhemorrhaging. biopolymer-based aerogels. Chitosan, cellulose alginate useful for wound wound healing and stopping Table presents summary for the theand biological characteristics as hemostatic properties, antibacterial and mucoadhesive properties which are useful for healing and stopping hemorrhaging. Table 11 presents aa summary for biological have been used in various medical applications due to their unique biological characteristics such as wound healing properties and molecular structures of chitosan, cellulose and alginates. These useful wound properties healing andand stopping hemorrhaging. 1 presents a summary the biological woundforhealing molecular structuresTable of chitosan, cellulose and for alginates. These hemostatic properties, antibacterial and mucoadhesive properties which are useful for wound healing biopolymers have been used used in tissue tissue engineering scaffolds, biosensing, medical implants, and drug wound healing properties and molecular structures of chitosan, cellulose andimplants, alginates. These biopolymers have been in engineering scaffolds, biosensing, medical and drug and stopping hemorrhaging. Table 1 presents a summary for the biological wound healing properties delivery . The chemistry of aerogels is very flexible and has been reported to be altered by many biopolymers been usedofinaerogels tissue engineering scaffolds, biosensing, medical drug delivery . have The chemistry is very flexible and has been reported to implants, be alteredand by many and molecular structures of chitosan, cellulose and alginates. These biopolymers have been used factors such as the precursor materials , their ratio , preparation approaches  and so on. Thein delivery . The chemistry of aerogels is very flexible and has been reported to be altered by many factors such as the precursor materials , their ratio , preparation approaches  and so on. The tissue engineering scaffolds, biosensing, implants, and drug delivery . chemistry pore size and theprecursor surface area of aerogels aerogels canratio also be tailored tailored .approaches The physical, physical, chemical andof factors such as the materials , medical their , preparation The and so on. The pore size and the surface area of can also be . The chemical and aerogels is very flexible and has been reported to be altered by many factors such as the precursor mechanical properties of aerogels mainly depend on the precursor material or group of materials that pore size and the surface area ofmainly aerogels can also beprecursor tailored . Theorphysical, mechanical properties of aerogels depend on the material group ofchemical materialsand that materials , their ratio , preparation approaches  and so on. The pore size and the surface form this network. mechanical properties of aerogels mainly depend on the precursor material or group of materials that form this network. areathis of aerogels form network.can also be tailored . The physical, chemical and mechanical properties of aerogels Table 1. Biological, Biological, wound healing properties and of molecular structures of this chitosan, cellulose and and mainly depend on the wound precursor material or group materials that form network. Table 1. healing properties and molecular structures of chitosan, cellulose alginate. Table 1. Biological, wound healing properties and molecular structures of chitosan, cellulose and alginate. Table 1. Biological, wound healing properties and molecular structures of chitosan, cellulose alginate. Biopolymer Biological Properties Properties Molecular Structure Structure References Biopolymer Biological Molecular References and alginate.
Biological Properties - Hemostatic agent due to positive charges that can bind to negative charges -charges Hemostatic agent duetotonegative positivecharges that can bind Hemostatic agent due to positive charges on red red blood blood cells.zhjAntibacterial and charges that can bind toAntibacterial negative charges on cells.zhjthat can bind to negative charges on and red Chitosan anti-fungal.zhjMucoadhesive on red blood cells.zhjAntibacterial and Chitosan anti-fungal.zhjblood cells. Mucoadhesive propertieszhjWound healing Chitosan Mucoadhesive Chitosan anti-fungal.zhj- Antibacterial and anti-fungal. propertieszhjWound healing acceleration and immune system - Mucoadhesive properties propertieszhjWound healing acceleration and immune system - Wound healing acceleration and immune stimulation. acceleration and immune system stimulation. system stimulation. stimulation. dueProperties to positive Biopolymer - Hemostatic agent Biological
High water water absorption absorption and and holding -- High - High water absorption andholding holding capacities.zhjGood wound exudates -capacities.zhjHigh water absorption and holding capacities. Good wound exudates Cellulose drainage capacity. zhjSupport and Good wound exudates Cellulose capacities.zhj- Goodcapacity. wound exudates drainage capacity. Cellulose drainage zhjSupport and enhance the growth and proliferation of Support and enhance the growth andof Cellulose drainage capacity. zhjSupport and enhance the growth and proliferation proliferation of cells. cells. enhance the growth and proliferation of cells. cells. - Preserving a solid-likeattribute attribute at Preserving solid-like at acidic acidic -- Preserving aa solid-like attribute at acidic conditions. conditions. zhjHemostatic properties, -conditions. Preservingzhja solid-like attribute at acidic Hemostatic properties, - Hemostatic properties, which are useful which are are useful useful for bleeding bleeding wounds.zhjconditions. zhjHemostatic properties, which for wounds.zhjAlginates for bleeding wounds. Alginates Alginates which Good mucoadhesive properties.zhjare useful for bleeding wounds.zhj- Good mucoadhesive properties. Good mucoadhesive properties.zhjAlginates Barrier protects immobilized material Barrier protects immobilized material Good mucoadhesive properties.zhjBarrier protects immobilized material toward physical stress. toward physical stress. Barrier material towardprotects physicalimmobilized stress. toward physical stress.
   
   
Antibiotics 2020, 9, 648
4 of 25
2.1. Chitosan-Based Aerogel Chitosan is one of the most abundant biopolymers on earth and has been extracted from multiple sources such as the shells of crustaceans , cell walls of fungi , and exoskeleton of arthropods  etc. The preparation of aerogels from polymeric nanoparticles such as chitosan is attracting increasing Antibiotics 2020, 9, x FOR PEER REVIEW 4 of 26 interest among scientists. The unique properties of resulted aerogels, such as high surface area, mechanical strength, a high degree of polymerization, high purity and high crystallinity make them 2.1. Chitosan-Based Aerogel promising materials for desired Chitosan has from beenmultiple reported to be Chitosan is onevarious of the most abundantapplications biopolymers on[35,36]. earth and has been extracted insoluble in watersuch and anofaqueous alkaline The, convenient mechanism resulting from sources asforms the shells crustaceans , cellsolution. walls of fungi and exoskeleton of arthropods  etc. The preparation aerogels allow from polymeric nanoparticles chitosan is attracting pH-dependent solubility of this of polymer its processing undersuch mildasconditions and the ability to increasing interest among scientists. The unique properties of resulted aerogels, such as high surface form various shapes and sizes of hydrogel or aerogel . Yi et al.  fabricated highly porous and area, mechanical strength, a high degree of polymerization, high purity and high crystallinity make anisotropicthem chitosan aerogels through directional freezing technology, which canreported sustaintoan promising materials for various desired applications [35,36]. Chitosan has been be extremely high compressive The authors reported that theThe chitosan aerogel was able to completely insoluble instrain. water and forms an aqueous alkaline solution. convenient mechanism resulting from pH-dependent solubility of the this polymer its processing under mild conditions the abilitya chitosan revert to its original height with release allow of imposed weight. Rinki et al. and fabricated to form various shapes and sizes of hydrogel or aerogel . Yi et al.  fabricated highly porous aerogel using supercritical carbon dioxide technique which exhibited a polymorphic mesoporous and anisotropic chitosan aerogels through directional freezing technology, which can sustain an structure. extremely The authors reported that theThe use of supercritical technique enhances high compressive strain. authors reported thatCO the 2chitosan aerogel was ablethe to porosity of aerogel.completely The structure changed nonporous and smooth to a porous and revert toofitsaerogel original height with from the release of imposed weight. Rinki structure et al.  fabricated a chitosan aerogel using supercritical dioxide which exhibited a polymorphic leaf-like structure. The surface area of thecarbon aerogel wastechnique in the mesoporous range. In another study, mesoporous structure. The authors reported that the use of supercritical CO2 technique enhances the Rubina et al.  prepared chitosan aerogel with a noticeably larger globule-like structure, as presented porosity of aerogel. The structure of aerogel changed from nonporous and smooth structure to a in Figure 2.porous In a different study, a comparison theofmechanical properties of a chitosan-based and leaf-like structure. The surfaceofarea the aerogel was in the mesoporous range. In aerogel was studied by Gómez et al. . their work,chitosan they compared the mechanical strength of the aerogel another study, Rubina et al.In  prepared aerogel with a noticeably larger globule-like structure, as presented Figure 2. In The a different study, a comparison thethe mechanical of after loading it with differentinmaterials. mechanical propertiesofof aerogelproperties were affected upon a chitosan-based aerogel was studied by Gómez et al. . In their work, they compared the loading the antibiotic (erythromycin), the aerogel showed crystalline deposits and a decrease in the mechanical strength of the aerogel after loading it with different materials. The mechanical properties hardness and Young’s unlike garlic extract(erythromycin), loaded aerogel, which showed of the aerogel modulus, were affected uponelephant loading the antibiotic the aerogel showed increase on the hardness and Young’s as showing texturization of elephant the micro sheets and crystalline deposits and amodulus, decrease in as thewell hardness and Young’s modulus, unlike garlic extract loaded aerogel, which showed increase on the hardness and Young’s modulus, as well as microfibers . This reveals that any addition to the aerogel may affect the morphology, mechanical showing texturization of the micro sheets and microfibers . This reveals that any addition to the strength, hardness and porosity. aerogel may affect the morphology, mechanical strength, hardness and porosity.
2. Scanning Electron Microscope images for the aerogel. Adapted from Rubina Figure 2. Figure Scanning Electron Microscope images forchitosan-based the chitosan-based aerogel. Adapted from et al. . Rubina et al. .
2.2. Cellulose-Based Aerogels
2.2. Cellulose-Based Aerogels
Cellulose is the most abundant biopolymer on earth and has been extracted from a variety of
Cellulose is the most abundant biopolymer on earth andofhas been extracted a variety of renewable and sustainable sources [41–43]. It is found in 9–25% plant primary cell wallsfrom and 40– 80% of their secondary cell walls. Cellulose also isolated from bacteria and some animals . renewable and sustainable sources [41–43]. It is found in 9–25% of plant primary cell walls and 40–80% Nanocellulose refers to nano-structured cellulose materials, which either cellulose nanocrystal (CNC) of their secondary cell walls. Cellulose also isolated from bacteria and some animals . Nanocellulose or cellulose nanofibre (CNF) . Both forms of cellulose have unique properties such as high surface refers to nano-structured materials, whichThese either cellulose or cellulose area, high strength,cellulose and tunable surface chemistry. properties arenanocrystal responsible for(CNC) controlled nanofibre (CNF) . Both forms of cellulose have unique properties as high surface interactions with other polymers, other nanoparticles, biological materialssuch or small molecules; thus,area, high strength, and tunable surface chemistry. These properties are responsible for controlled interactions with other polymers, other nanoparticles, biological materials or small molecules; thus, it is the most utilized biopolymer in different applications . The properties of cellulose-based aerogel differ based
Antibiotics 2020, 9, 648 Antibiotics 2020, 9, x FOR PEER REVIEW
5 of 25 5 of 26
on the CNF-based aerogel display more rice-shape morphology compared to the it materials is the mostused; utilized biopolymer in different applications . Theinproperties of cellulose-based spherical CNC aerogel. The shape of nanocellulose materials affects the appearance of aerogel aerogel differ based on the materials used; CNF-based aerogel display more rice-shape in . Zhang et al.  compared CNC and CNF aerogels and reported mixing morphology compared tothe theperformance spherical CNCof aerogel. The shape of nanocellulose materialsthat affects the the appearance of aerogel . Zhang et al. than  compared the performance CNC andofCNF aerogels two materials showed better performance the pure aerogel resulted of from each them. However, reported thatwere mixing the two materials showed better performance pure aerogel resulted all theand aerogels that prepared had a 3D network structure and than rich the in pores. Figure 3 presents from each of them. However, all the aerogels that were prepared had a 3D network structure and rich the obtained SEM images of the aerogels that were prepared by Zhang et al. . The morphology in pores. Figure 3 presents the obtained SEM images of the aerogels that were prepared by Zhang et result showed that CNC based aerogel is spherical while the CNF based aerogel showed rice-shape, al. . The morphology result showed that CNC based aerogel is spherical while the CNF based which resulted from the longer filament of CNF compared to CNC. The size, structure and morphology aerogel showed rice-shape, which resulted from the longer filament of CNF compared to CNC. The of aerogel pores can adjusted of byaerogel changing its the concentration or mixing size, structure andbe morphology poresthe canprecursor be adjustedmaterial, by changing precursor material, it with other particles. The mechanical properties of aerogel have been reported to be affected its concentration or mixing it with other particles. The mechanical properties of aerogel have been by two main factors: precursor material and preparation methodand . Yang et method al.  . reported reported to be affected by two main factors: precursor material preparation Yang that cellulose thethat mechanical properties the aerogel, and the of alginate cellulose et al.enhanced  reported cellulose enhanced theof mechanical properties of ratio the aerogel, and the ratio of had alginate effect cellulose significant effect on the mechanical properties. a different Zheng et the a significant onhad the amechanical properties. In a different study,In Zheng et al.study,  evaluated al.  evaluated the mechanical properties of cellulose aerogels by using CNC as reinforcement mechanical properties of cellulose aerogels by using CNC as reinforcement and concludedand that the concluded that the compressive modulus was significantly (6 times higher) compared to compressive modulus was significantly improved (6 timesimproved higher) compared to the pure cellulose the pure cellulose aerogel. Qin et al.  prepared cellulose-based aerogel with a specific surface area aerogel. Qin et al.  prepared cellulose-based aerogel with a specific surface area and a small amount and a small amount of mesopores. The authors evaluated the effect of loading Resveratrol drug into of mesopores. The authors evaluated the effect of loading Resveratrol drug into the aerogel and the aerogel and concluded that smaller amounts of pores in the aerogel appeared richer. Revealing concluded that smaller amounts of pores in the aerogelofappeared richer.resulted Revealing the appearance that the appearance of new pores and the changing pores diameter afterthat the addition of of new pores drug .and the changing of pores diameter resulted after the addition of drug .
Figure 3. Scanning Electron Microscope images 1:3 (cellulose nanocrystal/cellulose Figure 3. Scanning Electron Microscope images of (a) of mix(a)1:3mix (cellulose nanocrystal/cellulose nanofiber) nanofiber) (b) mix (c) mix(d) 3:1cellulose aerogel, nanocrystal (d) cellulose nanocrystal (e)nano aerogel, (b) mixaerogel, 1:1 aerogel, (c)1:1 mixaerogel, 3:1 aerogel, aerogel, (e)aerogel, cellulose cellulose nano fiber aerogel. Adapted from Zhang et al. . fiber aerogel. Adapted from Zhang et al. .
2.3. Alginate Based Aerogels 2.3. Alginate Based Aerogels Alginate a natural polymer mainlyobtained obtained from from brown seaweeds. It consists of of Alginate is a is natural polymer mainly brownalgae algaeand and seaweeds. It consists linear copolymers of β-(1–4) linked d-mannuronic acid and β-(1–4)-linked l-guluronic acid units . linear copolymers of β-(1–4) linked d-mannuronic acid and β-(1–4)-linked l-guluronic acid units . Sodium alginate is widely used thickening agent agent in andand antidote for heavy Sodium alginate is widely used asasa athickening inthe thefood foodindustry industry antidote for heavy metal ions in medicine . This anionic polysaccharide was able to cross-link with any divalent metal ions in medicine . This anionic polysaccharide was able to cross-link with any divalent 2+ and others. Alginate has been widely used in aerogel fabrication for many cation such as2+Ca2+, Zn 2+ cation such as Ca , Zn and others. Alginate has been widely used in aerogel fabrication for many medical  and non-medical applications . Alginate-based aerogels are reported to possess bulk densities, high surface areas and super absorbent behavior . They have the advantage of being easily processed from educts only by exchange of water, alcohol and carbon dioxide alone without the need
Antibiotics 2020, 9, 648
6 of 25
for other solvents, which is considered a safe alternative in terms of medical applications and wound dressing . Robitzer et al.  studied the organization at the nano-scale level of alginate-based aerogels, and it was concluded that morphology of the aerogel depends on the morphology of pre-existing objects within the gel, and any adjustment of the parent gel will affect the structure of the aerogel. The concentration of the polymeric solution is the main inference on the properties of aerogels. Baldino et al.  fabricated cylindrical shape alginate-based aerogels using supercritical drying technique. They studied the effect of polymer concentration on the physical and mechanical properties of aerogel. The authors reported that the morphology of aerogels changed from nano-fibrous to nano-porous when the alginate concentration increased as presented in Figure 4. The results of specific area values indicated that the lower alginate concentration, the higher specific area . Calcium alginate porous aerogels have been prepared in another study following the same technique of supercritical CO2 drying. It was observed that the aerogel from calcium alginate formed different pore sizes termed as micropores, macropores and surface area . The pore size of alginate-based aerogels was reported to be of nano-scale, in a recent study by Franco et al. . The characterization of calcium alginate aerogel showed that the aerogel had nano-porous structure using supercritical CO2 drying. Alginate/pectin aerogel microspheres were fabricated by Chen et al.  and revealed that higher alginate concentration presented higher stiffness and mechanical strength, while higher pectin concentration presented higher porosity and pore size. Antibiotics 2020, 9, x FOR PEER REVIEW
7 of 26
Figure 4. Internal section Scanning Electron Microscope images of: (a) 5% w/w Ca-Alginate aerogel,
Figure 4. Internal section Scanning Electron Microscope images of: (a) 5% w/w Ca-Alginate aerogel, (b) 5% w/w Cu-Alginate aerogel, (c) 10% w/w Ca-Alginate aerogel, (d) 10% w/w Cu-Alginate aerogel, (b) 5% w/w(e)Cu-Alginate aerogel, (c) 10% w/w aerogel, (d) 10% Cu-Alginate aerogel, 15% w/w Ca-Alginate aerogel, (f) 15% w/wCa-Alginate Cu-Alginate aerogel. Adapted from w/w Baldino et al. . (e) 15% w/w Ca-Alginate aerogel, (f) 15% w/w Cu-Alginate aerogel. Adapted from Baldino et al. . 2.4. Other Biopolymer-Based Aerogels Aerogel have been also fabricated from other biopolymers such as pectin , starch , carrageenan , agar , and xanthan [10,66]. Nešić et al. fabricated environmentally friendly pectin-based aerogel using TiO2 as an antibacterial agent. The authors compared the mechanical and thermal properties of pure pectin and pectin/TiO2 aerogels and revealed that the mechanical and thermal performance improved after the addition of metal oxide . Starch-based aerogels have been prepared from different sources such as corn, pea, tapioca and potato . Baudron et al. 
Antibiotics 2020, 9, 648
7 of 25
2.4. Other Biopolymer-Based Aerogels Aerogel have been also fabricated from other biopolymers such as pectin , starch , carrageenan , agar , and xanthan [10,66]. Neši´c et al. fabricated environmentally friendly pectin-based aerogel using TiO2 as an antibacterial agent. The authors compared the mechanical and thermal properties of pure pectin and pectin/TiO2 aerogels and revealed that the mechanical and thermal performance improved after the addition of metal oxide . Starch-based aerogels have been prepared from different sources such as corn, pea, tapioca and potato . Baudron et al.  recently prepared starch-based aerogel with particles size varied from 25 and 270 µm and Brunauer–Emmett–Teller (BET) surface area of 278 m2 /g. Agar has been extracted from red seaweeds, which mainly composed by two polysaccharides namely; agarose and agaropectin . Agar showed good compatibility with other biopolymers and it have been used to enhance the mechanical properties of starch based aerogels . Carrageenan is another naturally occurring polysaccharide was used in aerogel fabrication, Alnaief et al.  used micro-spherical carrageenan particles to fabricate biodegradable aerogel with a surface area ranged between 33 and 174 m2 /g, and an average pore 12.3 nm. 2.5. Biomedical Applications of Biopolymer-Based Aerogels Biopolymer-based aerogels have been extensively prepared, characterized and experimented for numerous biomedical applications due to their biocompatibility, lesser or non-cytotoxicity  and immunological response . Biopolymer has been utilized in biosensing, controlled drug release, tissue engineering scaffolds, skin and tissues repairs, etc. Aerogels have been used to overcome the issues associated with 1D and 2D materials in developing biosensors. Edwards et al.  used peptide-nano cellulose aerogels for biosensing. They fabricated an aerogel with high porosity to detect protease enzyme activity. The results of mass spectral analysis and the physical properties of prepared aerogel showed promising potential for wound dressing applications. A biosensor is an analytical device or material that can detect low concentrations of a desirable parameter . Cellulose nanocrystals aerogel has been fabricated to be able to detect human neutrophil elastase for healing chronic wounds . Biosensors, combined with certain biological components, form a physicochemical detector, which could be enzymatic or non-enzymatic based. Li et al.  successfully used chitosan-carbon nanotubes hybrid aerogel for non-enzymatic sensing. Peptide/cellulosic aerogel has been used as a micro-titer enzyme assay to determine the response, sensitivity, and kinetic behavior of the biosensor . Tissue engineering is another application of aerogel. Aerogel has been used for regeneration of various types of tissues such as skin, bones, cartilages and even blood vessels. Collagen-alginates aerogel has been evaluated for the regeneration of different tissues ; using bio-based materials has the advantage of being cytocompatible and non-toxic. Cellulose-based aerogel has been suggested to solve the issue of the potential complications associated with autografts. It has been widely used in tissue engineering scaffolds preparation. Osorio et al.  modified cellulose nanocrystal aerogels and used them as viable bone tissue scaffolds. Their findings demonstrated that cellulose-based aerogels are flexible, porous and facilitate bone growth after they are implanted in bone defects. Alginate/lignin nanocomposite aerogel has been evaluated for tissue scaffold. It possesses good cell adhesion properties and did not compromise cell viability . Using natural materials such as cellulose, alginates and chitosan in tissue scaffolds did not show any toxicity and, in most of the cases, enhanced the growth of cells. Kumari and Dutta  fabricated genipin-chitosan hybrid aerogel and evaluated its cytotoxicity. The porous structure of aerogel supported cell adhesion and proliferation. It was reported to be far less toxic than glutaraldehyde and safe for tissue engineering application. Controlled drug release at present has been at the forefront of research. Biopolymer-based aerogel has been proposed for use in controlled drug release. Rinki et al.  evaluated chitosan aerogel for potential drug delivery. The report of the study showed that the aerogel was biocompatible, non-cytotoxic, with intense antibacterial activity, making it suitable for drug delivery applications. Zhao et al.  used a combination of poly-ethylenimine grafted in cellulose nanofibril aerogels for drug
Antibiotics 2020, 9, 648
8 of 25
delivery. It was reported that the material is promising and proposed as a new generation of controlled drug delivery carriers. The unique pH and temperature-responsiveness together with their excellent physical, chemical, mechanical, biodegradability, biocompatibility and less cytotoxicity of biopolymers make them better than synthetic polymers. Alginate aerogel has also been reported to be suitable in mucosal drug delivery, mucoadhesive and non-cytotoxic . The presence of multi-functional groups on the surface of biopolymers and the advantage of the extremely high surface area of aerogel as material make them the right and desirable choice for drug delivery applications. 3. Biopolymer-Based Aerogels for Antibacterial Delivery Antibacterial delivery is one of the biomedical applications that has attracted a lot of research in the past few years. A significant number of publications have been published, and more research is still being conducted in this area. Drugs or natural antibacterial materials loading in the aerogel can be Antibiotics 2020, 9, x FOR PEER REVIEW 9 of 26 achieved either by adding them in the sol-gel process or in the post-processing of synthetic aerogels depending on the sensitivity of drugs and the fabrication techniques . Controlled release of loaded be achieved either by adding them in the sol-gel process or in the post-processing of synthetic antibacterial materials is essential. It has been reported that drug release is limited by the skeletal aerogels depending on the sensitivity of drugs and the fabrication techniques . Controlled release structure of the aerogel; such that the release rate decreases with the prolongation . of loaded antibacterial materials is essential. It has been reported that drug releaseofisrelease limitedtime by the Wang et al.structure  reported the change inthe therelease ratio ofrate ingredients thethe precursor materials would skeletal of thethat aerogel; such that decreases of with prolongation of release result in the aerogels with ordered pore structures and stable properties. In their research, the authors time . Wang et al.  reported that the change in the ratio of ingredients of the precursor were able to would controlresult the pore sizeaerogels by changing the concentration of theand polymer. Their resultInshowed materials in the with ordered pore structures stable properties. their thatresearch, higher concentration resulted smaller Furthermore, amount of drug the authors were able toin control thepore poresize. size by changing thethe concentration of thereleased polymer.by aerogel reported behigher dependent on the pore sizes.in smaller pore size. Furthermore, the amount Theirwas result showedto that concentration resulted Another major factor that affects drug release is the specific surface of drug released by aerogel was reported to be dependent on the pore sizes.area. The previous report major factor affects drug release the specific surface area. The report showedAnother that a change in the that specific area resulted inisa change in the dissolution rateprevious of the drug and showed that a change in the. specific area resulted in aaerogels change inhave the dissolution ratelarge of thesurface drug and drug absorption in the body Biopolymer-based an extremely area. drug absorption the body . Biopolymer-based aerogels have an extremely surface area. Thus, the adsorbedindrug in aerogels exhibited low dissolution properties, and islarge useful for the long Thus, the adsorbed drug in aerogels exhibited low dissolution properties, and is useful for the longon time delivery of drugs . The surface chemistry of biopolymer-based aerogels also had an impact of drugsHydrophilic . The surface chemistry biopolymer-based aerogels also had impact thetime rate delivery of drug release. aerogels possessofrapid drug release rate and serve as ananadvantage on the rate of drug release. Hydrophilic aerogels possess rapid drug release rate and serve as an for the controlled release of poor water-soluble drugs. However, hydrophobic aerogels, in contrast, advantage for the controlled release of poor water-soluble drugs. However, hydrophobic aerogels, in have a slower release rate, which is influenced by diffusion processes because they are more stable contrast, have a slower release rate, which is influenced by diffusion processes because they are more in water . The hydrophilicity of natural polymers can be altered using chemical compounds . stable in water . The hydrophilicity of natural polymers can be altered using chemical compounds The use of biopolymers as a carrier for different antibacterial substances including antibiotics , . The use of biopolymers as a carrier for different antibacterial substances including antibiotics essential oils , plant extracts , enzymes , metallic oxides  and nanoparticles has been , essential oils , plant extracts , enzymes , metallic oxides  and nanoparticles has done . Figure 5 presents a summary of the preparation process of antibacterial aerogel. been done . Figure 5 presents a summary of the preparation process of antibacterial aerogel.
Figure 5. Schematic drawing of biopolymers antibacterial aerogels. Figure 5. Schematic drawing of biopolymers antibacterial aerogels.
Since first aerogelwas wasproduced producedback backin in 1931, 1931, several several other forfor itsits Since thethe first aerogel othermaterials materialshave havebeen beenused used production and applied in different applications. Table 2 presents a summary of the chronological production and applied in different applications. Table 2 presents a summary of the chronological development of antibacterial aerogels since its first invention. The utilization of aerogels in antibacterial delivery began recently at the beginning of this century. Silver was first used as an antibacterial agent in the aerogel . The solution of silver nitrate (AgNO3) was used in the organic aerogels and reported to exhibit good antibacterial activity. Since then, various materials have been used as antibacterial activity as presented in Table 1.
Antibiotics 2020, 9, 648
9 of 25
development of antibacterial aerogels since its first invention. The utilization of aerogels in antibacterial delivery began recently at the beginning of this century. Silver was first used as an antibacterial agent in the aerogel . The solution of silver nitrate (AgNO3 ) was used in the organic aerogels and reported to exhibit good antibacterial activity. Since then, various materials have been used as antibacterial activity as presented in Table 1. Table 2. Chronological development of the antibacterial aerogels. Year
Type of Aerogels
Remark/Incorporated Antibacterial Material
1931 1968 1989 1997
Silica aerogel Metal oxide and silica Polymer aerogels Polymer aerogels
   
The first invention of aerogel. Development of sol-gel route for aerogel fabrication. Organic and carbon aerogel using sol-gel route. Ultralight aerogels using cross-linking techniques. Silver as antibacterial material and direct immersion of organic aerogels in aqueous AgNO3 solutions. The first use of silver nanoparticles for antibacterial properties in nanocellulose aerogel. Antibacterial mesoporous pure chitosan aerogels. Iron oxide and silver nanoparticles dispersed in nanofibrillated cellulose aerogel. Essential oils of medicinal plants used as antibacterial materials for air and surface disinfection. Lysozyme, Zinc oxide and gold nanoparticles immobilized in the cellulose network as antibacterial agents. Bacteriophage used as an antibacterial agent, which encapsulate within the cellulose fibers. Triclosan used as antibacterial material, in addition to improving the strength. Layer-by-layer surface-modified cellulose aerogel was able to adhere to bacterial cells from aquatic solutions. Lysozyme enzyme immobilized inside the cellulose aerogel as antibacterial material. Amoxicillin and gentamicin antibiotics loaded in the microcrystalline cellulose network. Vancomycin antibiotic-loaded inside the chitosan aerogel. Modified cellulose with N-isopropyl acrylamide, which used as an antibacterial agent after enduring chlorination. Essential oils as a natural antibacterial agent in the aerogel.
2008 2011 2013
Nanocellulose-based aerogel Chitosan aerogels Nanofibrillated cellulose aerogel
Cellulose diacetate fibers
Chitosan aerogel Bacterial cellulose aerogel Nanocellulose aerogel
     [92,99]     [103,104]   
3.1. Antibacterial Chitosan-Based Aerogels Chitosan has advantages over the other biopolymers in antibacterial activity due to the surface interaction between positively charged chitosan molecules and negatively charged membranes of microbial cells . Raafat et al.  investigated the interaction between chitosan and bacterial membranes under a transmission electron microscope. The authors were able to identify chitosan molecules “as vacuole-like” attached on bacteria cell surfaces, and these vacuoles made the cell membrane of the bacterial cell became locally detached from the cell wall. The interaction between chitosan molecules and microbial membranes mediated by the electrostatic forces between the protonated NH+3 groups presents within the molecules of chitosan and the negative residues, presumably by competing with Ca+2 for electronegative sites on the membrane surface . López-Iglesias et al.  evaluated the potential use of chitosan-based aerogel in delivering of vancomycin antibiotic for chronic wound management, and the loaded aerogel had unique properties (Figure 6). The authors reported that formation of aerogel enhanced air permeability and water sorption capacity of chitosan. The aerogel had high antibiotic content and fast drug release with enhanced antibacterial and cytocompatibility activities. Similarly, Wu et al.  loaded different antibiotics in chitosan aerogels. The ampicillin chitosan loaded aerogel exhibited strong antibacterial activity without any leaching. The authors also evaluated the in vitro cytotoxicity of their preparations using
Antibiotics 2020, 9, 648
10 of 25
human cells, and all the aerogel composites proved to be biocompatible. Furthermore, the in vivo rate wound model analysis showed that the aerogel could speed up wound healing efficiently . Antibiotics 2020, 9, x FOR PEER REVIEW
11 of 26
Figure 6. Properties of vancomycin-loaded chitosan aerogels, adapted from López-Iglesias et al. .
Figure 6. Properties of vancomycin-loaded chitosan aerogels, adapted from López-Iglesias et al. .
The synergistic antibacterial effect of the antibiotic and chitosan molecules give the aerogel The synergistic antibacterial effect of the antibiotic and chitosan molecules give the aerogel stronger antibacterial activity against all tested microorganisms. Unlike the other antibiotic-loaded stronger antibacterial activity against all tested microorganisms. Unlike the other antibiotic-loaded biopolymer-based aerogels, chitosan enhanced the impact of the antibiotics, giving strong biopolymer-based aerogels, enhanced impact of the antibiotics, giving have strong antibacterial antibacterial activity evenchitosan after decreasing the the dose. Chitosan aerogel microparticles been used activity decreasing thetreatment dose. Chitosan aerogel have been aused a drug carrier as aeven drugafter carrier for wound applications andmicroparticles were fabricated through newas procedure for wound applications and were fabricated through a new procedure .aerogel Jet cutting . Jettreatment cutting technique with supercritical drying is used to manufacture chitosan-based with excellent textural properties and release of antibacterial agents. Inaerogel a different study, technique with supercritical drying is controlled used to manufacture chitosan-based with excellent Gómez et al.  compared the antibacterial effect of chitosan-based aerogel when it was loaded with textural properties and controlled release of antibacterial agents. In a different study, Gómez et al.  the antibiotic erythromycin and of when it was loadedaerogel with elephant The antibacterial compared the antibacterial effect chitosan-based when garlic it wasextract. loaded with the antibiotic activity was measured prior to aerogel fabrication for both the antibiotic and elephant garlic extract. was erythromycin and when it was loaded with elephant garlic extract. The antibacterial activity The plant extract resulted inactive against all tested bacteria, even methicillin-resistant Staphylococcus measured prior to aerogel fabrication for both the antibiotic and elephant garlic extract. The plant aureus, compared to erythromycin, which did not show any activity against this strain. The release of extract resulted inactive against all tested bacteria, even methicillin-resistant Staphylococcus aureus, antibiotic from the aerogel to the agar was found to be dependent on the equilibrium forces with the compared to erythromycin, which did not show anycompounds activity against this strain. of antibiotic biopolymer; in contrast, the diffusion of the active of the plant extractThe was release not dependent fromon thethe aerogel to the agar was found to be dependent on the equilibrium forces with the biopolymer; biopolymer content revealing a week interaction between chitosan and the plant extract. Yang in contrast, the diffusion active compounds of the plant extract was not on the et al.  used chitosanofasthe a reinforcing agent with silver nanoparticles in micro and dependent nano cellulose aerogels;content both reinforcing well in the chitosan micro and nano cellulose aerogels, biopolymer revealing aagents week dispersed interaction between and the plant extract. Yangwhich et al.  antibacterial agent activity. usedexpressed chitosan great as a reinforcing with silver nanoparticles in micro and nano cellulose aerogels;
both reinforcing agents dispersed well in the micro and nano cellulose aerogels, which expressed great 3.2. Antibacterial Cellulose Based Aerogels antibacterial activity. Cellulose is the most used biopolymer carrier for different types of drugs; it has been used in
3.2. Antibacterial CellulosetoBased Aerogels antibacterial delivery deliver different metallic oxides such as silver nanoparticles , copper, zinc oxide , and titanium dioxide . The use of cellulose-based aerogel as the antibacterial Cellulose is the most used biopolymer carrier for different types of drugs; it has been used in carrier has been done by immobilizing or encapsulation of certain antibacterial material inside the antibacterial delivery[89,116]. to deliver different oxides such oils as silver nanoparticles , copper, cellulose network Various plantmetallic extracts and essential were reported to show strong zinc antibacterial oxide ,activity. and titanium dioxide . The use of cellulose-based aerogel as the antibacterial Punica granatum peels extract has been reported to have stronger antibacterial carrier has been immobilizing encapsulation antibacterial material inside the activity than done many by common antibioticsor. Using such of ancertain extract together with cellulose-based cellulose network Various extracts and essential oilsetwere reported show strong aerogel can be of[89,116]. great interest as an plant antibacterial aerogel. Darpentigny al.  used thistoprinciple. They extracted thymol, which is a natural compound from thyme that possesses strong antibacterial antibacterial activity. Punica granatum peels extract has been reported to have stronger antibacterial activity. authors impregnated thymol with cellulose produced with activity thanThe many common antibiotics . Using suchnanofibrils an extractand together withaerogel cellulose-based strong antibacterial activity against gram-positive and gram-negative bacteria. Similarly, Zhang et al. aerogel can be of great interest as an antibacterial aerogel. Darpentigny et al.  used this principle.
Antibiotics 2020, 9, 648
11 of 25
They extracted thymol, which is a natural compound from thyme that possesses strong antibacterial activity. The authors impregnated thymol with cellulose nanofibrils and produced aerogel with strong antibacterial activity against gram-positive and gram-negative bacteria. Similarly, Zhang et al.  used thyme essential oil in the cellulose-based aerogel, utilizing the advantage of having both antibacterial and antioxidant activity. The prepared aerogel exhibited good absorption capacity, good antibacterial activity, and sustained-release property. In another study, Khan et al.  used cellulose nanofibrils as aerogel matrix to immobilize silver nanoparticles and enzymes for antibacterial application. The authors tested their aerogel for potential use in clinical trials and it seemed to be non-toxic and biocompatible. Moreover, their report concluded that cellulose nanofibre is suitable to support for bioactive materials, effective in retaining enzymatic and antibacterial activities. The high cost of metallic nanoparticles limited their usage in research and prevented their commercialization. At present, most of the research is now focused on green alternatives such as plant extracts and/or essential oils. Amoxicillin is one of the most used antibiotics for bacterial infection treatment. However, due to many reasons, including the use of minimal or less inhibitory concentrations, many bacteria have developed resistance to this antibiotic. Shan et al.  loaded amoxicillin in cellulose aerogel with the aim of getting the better performance of the antibiotic when it is directly applied to the infected area. The loaded aerogels exhibited excellent antibacterial activity with prolonged release of the antibiotic. The ability of cellulose to cross-link with other materials and make many surface interactions with polar and even non-polar compounds enhanced its potential for different biomedical applications . A novel hybrid aerogel was fabricated by Zuguang et al. . The aerogel was obtained by modification of the crystalline region of cellulose using the oxidation of some functional groups. The modified cellulose is then cross-linked with silver nanoparticles as an antibacterial substance. The obtained aerogel showed a strong antibacterial effect against many bacterial species . Silver nanoparticles have been used as an antibacterial substance in many types of research, such as Salomoni et al., Tang et al., and Vijaya et al. [120–122], but due to some drawbacks, such as the costs and related health risks of silver nanoparticles, especially with high concentrations, meant they did not opt for large-scale industries . However, using the particles in combination with modified aerogels minimizes the required dose and immobilizes the particles to avoid their release in the bloodstream upon using the aerogel for wound dressing, and thus minimizes or prevents the potential toxicity. Another cellulose-based wet-stabilized aerogel has been fabricated by Henschen et al. , with the porous structure of their CNF aerogel retained after soaking in water. The surface of this aerogel was able to adhere to more than 99% of bacteria. The surface modifications that they made to the aerogel were the main reason for bacterial adherence, which was confirmed by microscopy analysis . Indicating the possibility of creating such 3D material able to high efficiency adsorb the bacteria, the high porosity, and thus great surface area of aerogel in combination with their open structure give the material potential for bacterial removal. The use of cellulose aerogels in antibacterial delivery has many environmental advantages of being green, sustainable, biodegradable, abundant, and non-environmentally taxing . As cellulose molecules contain the preponderance of hydroxyl functional groups, they tend to possesses a strong affinity to water . Water affinity or hydrophilicity of cellulose-based aerogel can be easily controlled, as it is able to crosslink with variety of different polarities of materials . Despite its inherent hydrophilicity, cellulose and cellulose-based materials have unparalleled advantages as a precursor for potential production of hydrophobic materials. This material has been widely used in self-cleaning, self-healing, oil and water separation, electromagnetic interference shielding, etc. . On the medical side, many studies evaluated the biocompatibility and cytotoxicity of cellulose-based aerogels [128–131], and it was concluded that no cytotoxicity has been observed with cellulose-based aerogels, confirming that they can be safely incorporated with antibacterial substances as a promising material for dressing and healing of wounds.
Antibiotics 2020, 9, 648
12 of 25
3.3. Antibacterial Alginates Based Aerogels Alginates can react with polyvalent metal cations such as sodium and calcium ions . These reactions often result in a 3D network of various materials such as hydrogels, microspheres, microcapsules, and aerogels. Martins et al.  evaluated the potential use of alginate aerogel in biomedical applications. Their report showed evidence of the high potential of these materials because of its biocompatibility and non-cytotoxicity. Unlike chitosan, this biopolymer does not exhibit any antibacterial activity, but it can form many surface interactions with different materials; thus, in most of the causes, alginate is used as a part of hybrid materials. Trucillo et al.  entrapped the antibiotic ampicillin loaded liposomes in alginate aerogels for prolonged drug release. The authors were able to make the release of antibiotic from the aerogel double the normal time. The multi free hydroxyl and carboxyl groups on the surface of alginate permit its cross-linking with several materials, which provides an outstanding candidate for antibacterial applications. Ma et al.  evaluated the potential use of alginate-based aerogel for wound dressing, using in vitro and in vivo methods. Their composite aerogels were formed from sodium alginate-graphene oxide and polyvinyl alcohol, in addition to norfloxacin, as an antibacterial material. The authors reported that the aerogel displayed excellent bioavailability of drug with sustained release behavior that was able to inhibit the growth of all tested bacteria. The aerogel enhanced the wound healing and promote the cell proliferation. Another alginate-based aerogel was formed by Raman et al. . The aerogel was designed to carry calcium, zinc, and silver cations, which possess antibacterial and effective anti-inflammatory activity. These cations were suspended all over the huge surface area of aerogel. This resulted in its good homogeneity and strong antibacterial activity. This result showed that proper homogenization of the solution containing all the needed materials or cations prior to aerogel fabrication is important in order to get a homogeneous aerogel. The carboxylate groups of the guluronate in alginate polymer cross-link with different cations, which are immobilized within the polymeric network. Alginate and pectin core-shell aerogel beads have been produced by De Cicco et al.  for prolonging drug activity on wounds. The broad-spectrum antibiotic Doxycycline was suspended and immobilized in these aerogels, which had surprisingly high drug encapsulation efficiency (of up to 87%). The authors reported that drug release was dependent on the concentration of alginate and on drug/pectin ratio. The ability of pectin to interact with doxycycline makes the concentration of this drug go into the core, which mainly contain the pectin not alginate, giving another advantage of using biopolymer blends in term of delivering different drugs. 3.4. Other Antibacterial Biopolymer-Based Aerogels Carrageenan has been incorporated with cellulose and silver nanoparticles to form an antibacterial aerogel for wound healing applications . Abdelgawad et al. used cellulose nanocrystals to enhance the mechanical properties of carrageenan aerogels and silver nanoparticles as antibacterial material. The release profile of the nanoparticles suggested that the aerogel showed good controlled and sustainable drug release. The aerogel was able to eliminate the growth of gram-positive and gram-negative bacteria, i.e., Staphylococcus aureus and Escherichia coli, respectively. Similarly, Shen et al.  successfully utilized bagasse to fabricate ultra-light aerogel, with silver nanoparticles as an antibacterial agent. The obtained aerogel exhibited a strong antibacterial effect, especially against E. coli and Pseudomonas aeruginosa. In a different study, pectin-based nanocomposite aerogels were fabricated for potential food packaging applications . The authors’ incorporated titanium dioxide in the aerogel, and it displayed strong antibacterial activity against E. coli. Nisar et al.  used clove bud essential oil as antibacterial and antioxidant material in citrus pectin films. The inclusion of the essential oil significantly enhanced the water barrier properties of the films. However, the film showed complete growth of three common foodborne bacteria.
Antibiotics 2020, 9, 648
13 of 25
4. The Role of Biopolymer-Based Aerogel in Wound Healing Applications Bacterial infections have been a major public health challenge associated with wounds and the leading cause of death. It has been reported that 1 out of 2% of the population in developed countries have suffered from a chronic wound in their lifetime, and this is even more for less developed countries [138,139]. In 2018, Sen  studied the estimated cost of human wounds and their burden. Sen reported that medicare cost projections for all wounds types ranged from $28.1 billion to $96.8 billion, including costs for infection management. The author also added that there was significant demand for wound care products. Globally, the annual average cost for wound care was $2.8 billion in 2014, and it will jump to $3.5 billion in 2021 . In the design of wound dressings, preventing the infection is as important as stopping hemorrhaging and absorbing the wound exudates. Potential material must enhance cell proliferation, be easy to handle, biodegradable, permit gas exchange and be non-cytotoxic . Being deprived of adequate oxygen, known as hypoxia, is one of the main factors hindering the process of wound healing, resulting in chronic wounds . Contrasting many wound dressing materials, aerogel, with its high porosity, allows oxygen permeability, which is necessary for the normal healing process . Hydrogel has been used in wound treatment as an antibacterial carrier and has been prepared from different polymeric materials . Table 3 presents comparisons between hydrogels and aerogels in terms of antibacterial and wound healing applications. Table 3. Comparison between hydrogel and aerogel in wound healing applications. Functionality
Fluids absorption in wet wounds
Does not absorb fluids and cannot be used in wet wounds.
Able to absorb large amounts of fluids in wet wounds. Can be used to absorb fluid and expand to fill the wound. Excellent mechanical strength and easy to handle. The high porosity of aerogels provides suitable aeration for wounds. Lower cytotoxicity. Easy for patients to change their dressings. Higher cost of production.
Mechanical stability Wounds aeration Potential cytotoxicity Reliability for patients Cost of production
Poor mechanical strength and liable to tearing easily. Does not provide aeration to wounds. Relatively higher Difficult for patients to change their dressings. Lower cost of production.
Reference [145,146]      
Over 300 wound dressing forms have been developed, but most of them have common problems associated with their poor absorption of wound exudates, poor gas exchange, lack of antibacterial activity, difficulty in removing and handling, and non-sterile and allergic reactions . Traditional wound dressing materials are designed to keep the wounds dry and warm, such as absorbent pad, gauzes and felt . One of the biggest issues associated with traditional dressings is the adherence structure, which sometimes causes real trauma to patients due to their difficulty to remove from the wound surface. However, some traditional dressings possess low adherence, such as those with polyamide contact layer . Bacterial infection can possibly occur if no disinfection is used or the wound was not clean from microorganisms. Extensible bandages, cotton and rubber elastic bandages, elastic web bandages, elastic adhesive bandages, and rubber elastic are few examples of traditional wound dressing materials . The unique properties of biopolymer-based antibacterial aerogels make them potential materials that can overcome all the problems associated with currently used wound dressing. Biopolymer-based aerogel have excellent absorption ability of wound exudates, strong antibacterial activity, and reduce adverse allergic effects. Furthermore, they are biocompatible and non-immunogenic; these properties improve the wounds healing process. Figure 7 presents comparative schematic drawings of using conventional wounds dressing and antibacterial aerogels.
Antibiotics 2020, 9, 648 Antibiotics 2020, 9, x FOR PEER REVIEW
14 of 25 15 of 26
Figure 7. Schematic drawing of conventional dressing materials and antibacterial aerogel. Figure 7. Schematic drawing of conventional dressing materials and antibacterial aerogel.
Various antibacterialaerogels aerogels composites composites have applications . Various antibacterial have been beenused usedininwound woundhealing healing applications . The ability of these aerogels to absorb water has been utilized in wound healing as small injectable The ability of these aerogels to absorb water has been utilized in wound healing as small injectable pieces of aerogel, which can stop the bleeding of the deep wound and prevent bacterial infection at pieces of aerogel, which can stop the bleeding of the deep wound and prevent bacterial infection at the same time. Recently, Fan et al.  fabricated an injectable aerogel composite for this purpose. the same time. Recently, Fan et al.  fabricated an injectable aerogel composite for this purpose. The aerogel was composed of oxidized cellulose nanofiber to provide the physical and mechanical The aerogel was composed of oxidized cellulose nanofiber to provide the physical and mechanical properties and chitosan for rapid hemostasis of non-compressible hemorrhage application, as Figure properties and chitosan for rapid hemostasis of non-compressible hemorrhage application, as Figure 8a 8a presents. Unlike traditional wound dressing materials, using biodegradable and bioresorbablepresents. Unlike traditional wound dressing materials, usingtobiodegradable and bioresorbable-based based materials means that no further surgery is required remove the products, because these materials means that no further surgery is required to remove the products, because these materials materials are biodegradable, and some studies reported that they slowly degrade and are ultimately areabsorbed biodegradable, and some studies reported that they slowly degrade and are ultimately absorbed by the tissues in the body without any side effects [158,159]. Chitosan enhances the by theproduction tissues in the body side effects [158,159]. Chitosan enhances the production of type of type IIIwithout collagenany production from the human cells around the wound environment, in III collagen production fromthe theproliferation human cellsand around the wound environment, to the improving addition to improving migration of fibroblasts. Thus it in is addition considered right thechoice proliferation and migration of fibroblasts. it is considered the right ingrade wound healing in wound healing materials as it has allThus the properties that promote thechoice healing . materials as it has all the properties that promote the healing grade . In a different study, Batista et al.  developed a new preparation route for hybrid alginate-chitosan aerogel for wound healing applications. The authors observed no cytotoxic effect for the aerogel produced. The aerogel enhances wound recovery scratch compared with the control. It also possesses clear antibacterial activity against gram-positive and gram-negative bacteria. Surface modification of biopolymers has been reported to enhance its water absorption ability . To enhance the absorption, Fan et al. used carboxyl groups to modify cellulose nanofiber with high-pressure homogenization and then reacted with the amidogen of chitosan to fabricate the injectable aerogels composites. These aerogels were observed to absorb the blood and rapidly expand to fill the wound area (Figure 8a,b) . The aerogel had rapid shape recovery and good antibacterial ability due to the interaction between the two polymers and chitosan. However, this antibacterial activity could be significantly enhanced by the addition of an extra natural antibacterial material such as plant extract or essential oil. Cellulose/chitosan aerogel composite has been reported to be biocompatible and non-toxic to cells, with good adhesion and aggregation effect to red blood cells and platelets [2,149]. This is the same as many essential oils, which have been reported to have wound healing ability, antibacterial and antioxidant activities . Alginate-chitosan aerogel is another composite aerogel that has been recently developed by Batista et al. . The composite aerogel mix can provide a
Antibiotics 2020, 9, 648
15 of 25
moisty environment for the alginate with the antibacterial activity of chitosan. These two factors are essential for the wound healing process. The composite aerogels were evaluated for potential use in the wound healing procedure. These composites were reported to be non-cytotoxic, biocompatible, and enhanced the closing of the wound area higher than the untreated control. The result showed that the combination of a biopolymer has great potential for wound healing applications . In another study, Franco et al.  impregnated the mucopolysaccharide complex (Mesoglycan) onto calcium alginate aerogel. This is to produce novel material for re-epithelialization in the wound healing process. In vitro wound healing analysis confirmed that the aerogel composite increases the migration rate on fibroblast cells and enhances the proliferation of cells, which was observed from the result of covered distance for keratinocytes . Biranje et al.  used chitosan/seaweed aerogel composite for wound dressing to promote hemostasis of the wounds and tissue growth, which is required during hemorrhaging. In vitro evaluation of hemostatic properties was done using human thrombin-anti-thrombin assay. The aerogel showed steady blood coagulation and adhesion of platelet and red blood cells, which helped in the formation of thrombin. The authors concluded that their dressing aerogel accelerated hemostatic activity against hemorrhaging. Chitosan-based aerogels and films have been fabricated for immediate hemorrhage control . The aerogel exhibited mechanical strength, excellent fluid absorption, and improved blood clotting capacity. The authors performed intracellular reactive oxygen species assay and concluded that bacterial death resulted from damaging the cells. Similarly, chitosan/cellulose composite aerogel has been evaluated by Fan et al.  for massive hemorrhage control, which exhibited high water absorption capacity, excellent antibacterial activity, and rapid shape recoverability. The authors added that the developed aerogel had better coagulation ability than many traditional gauzes and gelatin sponge. Furthermore, the in vivo study showed rapid hemostasis, better biocompatibility, and no cytotoxicity was observed . In summary, three-dimensional biopolymer-based aerogels have been reported as an ideal candidate to replace traditional wound dressings. Some previous studies in this area showed that biopolymer-based aerogel has an excellent potential for antibacterial delivery for superficial wound dressing and injectable for to stop hemorrhage. Antibiotics 2020, 9, x FOR PEER REVIEW
16 of 26
Figure8. 8.(a)(a) Schematic illustration simulating injection aerogel composites wound, (b) Figure Schematic illustration of of simulating injection aerogel composites intointo the the wound, (b) digital digital photos of aerogel with rapid shape recovery after water absorption. Adapted from Fan et al. photos of aerogel with rapid shape recovery after water absorption. Adapted from Fan et al. . .
In a different study, Batista et al.  developed a new preparation route for hybrid alginatechitosan aerogel for wound healing applications. The authors observed no cytotoxic effect for the aerogel produced. The aerogel enhances wound recovery scratch compared with the control. It also possesses clear antibacterial activity against gram-positive and gram-negative bacteria. Surface
Antibiotics 2020, 9, 648
16 of 25
The wound healing process is a multi-factorial physiological process; the complexity of its different phases and undesired abnormalities could make the healing process very difficult. The wound dressing is designed to prevent bacterial infection because this is one of the most important external effectors during the healing process of wounds. There is a growing interest in developing smart wound dressings characterizes with: self-sterilization and inhibition of bacterial invasion, bio-adhesiveness to the wound surface, ease of application, biodegradability, oxygen permeability, and non-toxicity, etc. The current biopolymer-based antibacterial aerogels have the potential to be the first option in wound dressing to prevent the chronicity of wounds and enhance the quality of patients’ lives. The in vivo results of many studies in term of antibacterial wound healing and stopping hemorrhaging are promising for many wound healing applications. 5. Challenges and Propositions of Biopolymer-Based Antibacterial Aerogels The multi-functional groups surface modification of biopolymers and the high surface area of nanomaterial aerogels give the nano biopolymer-based aerogels tremendous ability to form cross-links with different functional groups. Little research has been done regarding the incorporation of plant extracts and/or essential oils in aerogels. However, the investigations of the antibacterial activity of many essential oils, plants aquatic and alcoholic extracts has been done, and many of them proved their strong antibacterial activity. In alternative medicine, plant extracts and essential oils have been reported to have hemostasis ability as well as antimicrobial and antioxidant activity . Antibacterial cellulose-based edible films have been fabricated for food packaging applications by using thyme essential oil as an antibacterial ingredient inside the film . The essential oil forms many cross-links all along the surface of cellulose film, giving the film the antibacterial character and keeping the physicochemical and mechanical properties of cellulose film. The same strategy could be followed in biopolymer-based aerogels, and the huge surface area of this material, numerous properties, such as antibacterial, antioxidant, and/or anti-inflammatory substances could be integrated inside these aerogels. The same principle would be helpful in developing chronic diabetic wound sheets; the air permeability of aerogel will provide extensive oxygen on the surface of the wound, preventing the growth of anaerobic bacteria, which is the main cause of gangrene . Antibacterial aerogels will provide clean wounds and inhibit the aerobic bacterial growing, without closing or preventing the aeration, which is necessary for wound healing . The large-scale production and commercialization of biopolymer-based antibacterial aerogels have not yet started. It is still in pre-clinical and clinical evaluation. As wound dressing is of high demand, the cost of production of biopolymer-based antibacterial aerogel will be reduced compared to the conventional material because all the logistics, environmental issues and post wound healing costs would have been eliminated. Furthermore, that large-scale production of biopolymer-based antibacterial aerogels will significantly lower the cost of production. However, in order to propose the safe use of biopolymer-based aerogels for any medical application, it is important to evaluate short-term as well as long-term toxicity and fate of these materials. Recently, some authors raised important concerns that justify the study of bio-interactions and the possible impact on humans upon the exposure to nanocellulose materials [169–171]. This would provide consistent and useful knowledge that can guide the outgrowth of regulations. Most of past and current health impact evaluations have been studied by the determination of the viability and cytotoxicity of the material on animal or human cell lines. However, this is done without considering the chronic effect of the material during the long-term exposure or exacerbation of pre-existing disease conditions. Furthermore, such studies have not been conducted on the cytotoxicity of reported potential blends of biopolymer-based aerogel. Different fabrication techniques, in most cases, have been followed using different chemicals and procedures, raising another concern about the effect of each technique on the antibacterial functionality of the developed material. The intensity of concerns about the developing of antibiotic resistance has depended on various factors, including bacterial exposure to different materials. Yahya et al.  evaluated the effect of some natural materials on the antibiotic sensitivity
Antibiotics 2020, 9, 648
17 of 25
of bacteria and concluded a significant increase upon the exposure. Pan et al.  reported that some metal nanoparticles induced mutagenic effect on bacterial cells. The effect of microbial exposure to nano polymer-based materials is still under research and not yet been determined. Further studies are needed on the effect of biopolymer-based aerogels on the microorganisms, to determine the potential mutagenic induction. 6. Conclusions This review has critically analyzed the properties of three biopolymer-based aerogels used in antibacterial delivery and highlighted the most recent works exploring the utilization of these aerogels in wound healing and skin tissue repair applications. Biopolymer-based aerogels based on previous studies have provided a potential platform to cross-link with a large variety of antibacterial materials to exploit new forms of functional materials. The quality of wound treatment process, especially chronic wounds, have been proposed for improvement using biopolymer-based aerogel. Biopolymer-based aerogels are suitable for these biomedical applications due to their ability to be incorporated with different antibacterial materials, resulting in aerogels with antibacterial properties. The utilization of antibacterial biopolymer-based aerogels in wound healing applications has been steadily raised due to the increasing demand for safer medical solutions in term of chronic wound healing, stopping hemorrhaging and enhance cell proliferation and tissue repair. Many studies have confirmed that biopolymer-based aerogels are biocompatible, non-cytotoxic and do not cause any immune reaction. However, much work is still needed in the application of the aerogel to different types of wound. Furthermore, different body allergies need to be considered before its commercialization. Author Contributions: Conceptualisation, H.P.S.A.K., E.B.Y., and F.J.; Methodology, H.P.S.A.K. and E.B.Y.; Software, N.G.O., C.K.A.; Validation, A.S.A., A.A.A., and S.R.; Formal analysis, E.B.Y., M.K.M.H. and N.G.O.; Investigation, H.P.S.A.K., E.B.Y., and F.J.; Resources, A.A.A., C.K.A., and A.S.A.; Data. H.P.S.A.K. and E.B.Y.; Writing—original draft preparation H.P.S.A.K., E.B.Y., and F.J.; Writing—review and editing, H.P.S.A.K., E.B.Y., and F.J.; Supervision H.P.S.A.K., A.A.A., and F.J.; Funding acquisition, H.P.S.A.K. and F.J. All authors have read and agreed to the published version of the manuscript. Funding: This work was financially supported by the Ministry of Higher Education, FRGS-MRSA 203.PTEKIND.6711837. Acknowledgments: The authors would like to thank the collaboration between the Management Science University Medical Centre, Selangor, Malaysia; Universitas Syiah Kuala, Banda Aceh, Indonesia; and the Universiti Sains Malaysia, Penang, Malaysia that made this work possible. Conflicts of Interest: The authors declare no conflict of interest.
References 1. 2.
De France, K.J.; Hoare, T.; Cranston, E.D. Review of hydrogels and aerogels containing nanocellulose. Chem. Mater. 2017, 29, 4609–4631. [CrossRef] Abdul Khalil, H.P.S.; Adnan, A.; Yahya, E.B.; Olaiya, N.; Safrida, S.; Hossain, M.; Balakrishnan, V.; Gopakumar, D.A.; Abdullah, C.; Oyekanmi, A. A Review on Plant Cellulose Nanofibre-Based Aerogels for Biomedical Applications. Polymers 2020, 12, 1759. [CrossRef] [PubMed] Ziegler, C.; Wolf, A.; Liu, W.; Herrmann, A.K.; Gaponik, N.; Eychmüller, A. Modern inorganic aerogels. Angew. Chem. Int. Ed. 2017, 56, 13200–13221. [CrossRef] [PubMed] Surya, I.; Olaiya, N.; Rizal, S.; Zein, I.; Sri Aprilia, N.; Hasan, M.; Yahya, E.B.; Sadasivuni, K.; Abdul Khalil, H.P.S. Plasticizer enhancement on the miscibility and thermomechanical properties of polylactic acid-chitin-starch composites. Polymers 2020, 12, 115. [CrossRef] Tamer, T.M.; Collins, M.N.; Valachová, K.; Hassan, M.A.; Omer, A.M.; Mohy-Eldin, M.S.; Švík, K.; Jurˇcík, R.; Ondruška, L’.; Biró, C. MitoQ loaded chitosan-hyaluronan composite membranes for wound healing. Materials 2018, 11, 569. [CrossRef] Abdul Khalil, H.P.S.; Jummaat, F.; Yahya, E.B.; Olaiya, N.; Adnan, A.; Abdat, M.; NAM, N.; Halim, A.S.; Kumar, U.; Bairwan, R. A review on micro-to nanocellulose biopolymer scaffold forming for tissue engineering applications. Polymers 2020, 12, 2043. [CrossRef]
Antibiotics 2020, 9, 648
9. 10. 11. 12.
13. 14. 15. 16.
18. 19. 20. 21.
22. 23. 24.
25. 26. 27.
18 of 25
Subrahmanyam, R.; Gurikov, P.; Dieringer, P.; Sun, M.; Smirnova, I. On the road to biopolymer aerogels—Dealing with the solvent. Gels 2015, 1, 291–313. [CrossRef] Maleki, H.; Durães, L.; García-González, C.A.; del Gaudio, P.; Portugal, A.; Mahmoudi, M. Synthesis and biomedical applications of aerogels: Possibilities and challenges. Adv. Colloid Interface Sci. 2016, 236, 1–27. [CrossRef] Subrahmanyam, R.; Gurikov, P.; Meissner, I.; Smirnova, I. Preparation of biopolymer aerogels using green solvents. JoVE 2016, 113, e54116. [CrossRef] Zhao, S.; Malfait, W.J.; Guerrero-Alburquerque, N.; Koebel, M.M.; Nyström, G. Biopolymer aerogels and foams: Chemistry, properties, and applications. Angew. Chem. Int. Ed. 2018, 57, 7580–7608. [CrossRef] Long, L.-Y.; Weng, Y.-X.; Wang, Y.-Z. Cellulose aerogels: Synthesis, applications, and prospects. Polymers 2018, 10, 623. [CrossRef] [PubMed] García-González, C.A.; Budtova, T.; Durães, L.; Erkey, C.; Del Gaudio, P.; Gurikov, P.; Koebel, M.; Liebner, F.; Neagu, M.; Smirnova, I. An opinion paper on aerogels for biomedical and environmental applications. Molecules 2019, 24, 1815. [CrossRef] [PubMed] Rebelo, R.; Fernandes, M.; Fangueiro, R. Biopolymers in medical implants: A brief review. Procedia Eng. 2017, 200, 236–243. [CrossRef] Kistler, S.S. Coherent expanded aerogels and jellies. Nature 1931, 127, 741. [CrossRef] Berardi, U.; Zaidi, S.M. Characterization of commercial aerogel-enhanced blankets obtained with supercritical drying and of a new ambient pressure drying blanket. Energy Build. 2019, 198, 542–552. [CrossRef] Chen, Y.; Zhou, L.; Chen, L.; Duan, G.; Mei, C.; Huang, C.; Han, J.; Jiang, S. Anisotropic nanocellulose aerogels with ordered structures fabricated by directional freeze-drying for fast liquid transport. Cellulose 2019, 26, 6653–6667. [CrossRef] Mi, H.-Y.; Jing, X.; Liu, Y.; Li, L.; Li, H.; Peng, X.-F.; Zhou, H. Highly durable superhydrophobic polymer foams fabricated by extrusion and supercritical CO2 foaming for selective oil absorption. ACS Appl. Mater. Interfaces 2019, 11, 7479–7487. [CrossRef] Pirzada, T.; Ashrafi, Z.; Xie, W.; Khan, S.A. Cellulose Silica Hybrid Nanofiber Aerogels: From Sol–Gel Electrospun Nanofibers to Multifunctional Aerogels. Adv. Funct. Mater. 2020, 30, 1907359. [CrossRef] Liu, R.; Wang, J.; Du, Y.; Liao, J.; Zhang, X. Phase-separation induced synthesis of superhydrophobic silica aerogel powders and granules. J. Solid State Chem. 2019, 279, 120971. [CrossRef] Yuan, B.; Zhou, S.-Y.; Chen, X.-S. Rapid prototyping technology and its application in bone tissue engineering. J. Zhejiang Univ. Sci. B 2017, 18, 303–315. [CrossRef] Tang, A.; Li, J.; Li, J.; Zhao, S.; Liu, W.; Liu, T.; Wang, J.; Liu, Y. Nanocellulose/PEGDA aerogel scaffolds with tunable modulus prepared by stereolithography for three-dimensional cell culture. J. Biomater. Sci. Polym. Ed. 2019, 30, 797–814. [CrossRef] [PubMed] Zhang, D.; Liu, X.; Qiu, J. 3D printing of glass by additive manufacturing techniques: A review. Front. Optoelectron. 2020, 13, 1–15. [CrossRef] Saoud, K.M.; Saeed, S.; Bertino, M.F.; White, L.S. Fabrication of strong and ultra-lightweight silica-based aerogel materials with tailored properties. J. Porous Mater. 2018, 25, 511–520. [CrossRef] Kam, D.; Chasnitsky, M.; Nowogrodski, C.; Braslavsky, I.; Abitbol, T.; Magdassi, S.; Shoseyov, O. Direct cryo writing of aerogels via 3d printing of aligned cellulose nanocrystals inspired by the plant cell wall. Colloids Interfaces 2019, 3, 46. [CrossRef] Jiang, Y.; Xu, Z.; Huang, T.; Liu, Y.; Guo, F.; Xi, J.; Gao, W.; Gao, C. Direct 3D printing of ultralight graphene oxide aerogel microlattices. Adv. Funct. Mater. 2018, 28, 1707024. [CrossRef] Alnaief, M.; Obaidat, R.; Mashaqbeh, H. Effect of processing parameters on preparation of carrageenan aerogel microparticles. Carbohydr. Polym. 2018, 180, 264–275. [CrossRef] Arenillas, A.; Menéndez, J.A.; Reichenauer, G.; Celzard, A.; Fierro, V.; Hodar, F.J.M.; Bailón-Garcia, E.; Job, N. Properties of carbon aerogels and their organic precursors. In Organic and Carbon Gels; Springer: Berlin/Heidelberg, Germany, 2019; pp. 87–121. Hu, L.; He, R.; Lu, Z.; Zhang, K.; Bai, X. Step-freeze-drying method for carbon aerogels: A study of the effects on microstructure and mechanical property. RSC Adv. 2019, 9, 9931–9936. [CrossRef] Bano, I.; Arshad, M.; Yasin, T.; Ghauri, M.A.; Younus, M. Chitosan: A potential biopolymer for wound management. Int. J. Biol. Macromol. 2017, 102, 380–383. [CrossRef]
Antibiotics 2020, 9, 648
30. 31. 32. 33. 34. 35.
41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51.
19 of 25
Portela, R.; Leal, C.R.; Almeida, P.L.; Sobral, R.G. Bacterial cellulose: A versatile biopolymer for wound dressing applications. Microb. Biotechnol. 2019, 12, 586–610. [CrossRef] Draget, K.I.; Taylor, C. Chemical, physical and biological properties of alginates and their biomedical implications. Food Hydrocoll. 2011, 25, 251–256. [CrossRef] El Knidri, H.; Belaabed, R.; Addaou, A.; Laajeb, A.; Lahsini, A. Extraction, chemical modification and characterization of chitin and chitosan. Int. J. Biol. Macromol. 2018, 120, 1181–1189. [CrossRef] [PubMed] Zamani, A. Superabsorbent Polymers from the Cell Wall of Zygomycetes Fungi. Ph.D. Thesis, Chalmers University of Technology, Gothenburg, Sweden, 2010. Ambarish, C.N.; Sridhar, K.R. Isolation and characterization of chitin from exoskeleton of pill-millipedes. Trends Biomater. Artif. Organs 2015, 29, 155–159. Zhang, Z.; Sèbe, G.; Rentsch, D.; Zimmermann, T.; Tingaut, P. Ultralightweight and flexible silylated nanocellulose sponges for the selective removal of oil from water. Chem. Mater. 2014, 26, 2659–2668. [CrossRef] Nuryawan, A.; Abdullah, C.; Hazwan, C.M.; Olaiya, N.; Yahya, E.B.; Risnasari, I.; Masruchin, N.; Baharudin, M.; Khalid, H.; Abdul Khalil, H.P.S. Enhancement of oil palm waste nanoparticles on the properties and characterization of hybrid plywood biocomposites. Polymers 2020, 12, 1007. [CrossRef] [PubMed] Rinki, K.; Dutta, P.K.; Hunt, A.J.; Macquarrie, D.J.; Clark, J.H. Chitosan aerogels exhibiting high surface area for biomedical application: Preparation, characterization, and antibacterial study. Int. J. Polym. Mater. 2011, 60, 988–999. [CrossRef] Yi, L.; Yang, J.; Fang, X.; Xia, Y.; Zhao, L.; Wu, H.; Guo, S. Facile fabrication of wood-inspired aerogel from chitosan for efficient removal of oil from water. J. Hazard. Mater. 2020, 385, 121507. [CrossRef] Rubina, M.S.; Elmanovich, I.V.; Shulenina, A.V.; Peters, G.S.; Svetogorov, R.D.; Egorov, A.A.; Naumkin, A.V.; Vasil’kov, A.Y. Chitosan aerogel containing silver nanoparticles: From metal-chitosan powder to porous material. Polym. Test. 2020, 86, 106481. [CrossRef] Gómez, M.A.; Bonilla, J.M.; Coronel, M.A.; Martínez, J.; Morán-Trujillo, L.; Orellana, S.L.; Vidal, A.; Giacaman, A.; Morales, C.; Torres-Gallegos, C. Antibacterial activity against Staphylococcus aureus of chitosan/chondroitin sulfate nanocomplex aerogels alone and enriched with erythromycin and elephant garlic (Allium ampeloprasum L. var. ampeloprasum) extract. Pure Appl. Chem. 2018, 90, 885–900. Yazdanbakhsh, M.; Rashidi, A.; Rahimi, M.; Khajavi, R.; Shafaroodi, H. Alpha-cellulose extraction from wheat bran for preparing cellulose nanofibers. Am. J. Oil Chem. Technol. 2017, 5, 46–52. Manzato, L.; Takeno, M.L.; Pessoa-Junior, W.A.G.; Mariuba, L.A.M.; Simonsen, J. Optimization of cellulose extraction from jute fiber by Box-Behnken design. Fibers Polym. 2018, 19, 289–296. [CrossRef] Meng, F.; Zhang, X.; Yu, W.; Zhang, Y. Kinetic analysis of cellulose extraction from banana pseudo-stem by liquefaction in polyhydric alcohols. Ind. Crops Prod. 2019, 137, 377–385. [CrossRef] Madsen, B.; Gamstedt, E.K. Wood versus plant fibers: Similarities and differences in composite applications. Adv. Mater. Sci. Eng. 2013, 2013, 564346. [CrossRef] Phanthong, P.; Reubroycharoen, P.; Hao, X.; Xu, G.; Abudula, A.; Guan, G. Nanocellulose: Extraction and application. Carbon Resour. Convers. 2018, 1, 32–43. [CrossRef] Lavoine, N.; Bergström, L. Nanocellulose-based foams and aerogels: Processing, properties, and applications. J. Mater. Chem. A 2017, 5, 16105–16117. [CrossRef] Zhang, T.; Zhang, Y.; Wang, X.; Liu, S.; Yao, Y. Characterization of the nano-cellulose aerogel from mixing CNF and CNC with different ratio. Mater. Lett. 2018, 229, 103–106. [CrossRef] Simón-Herrero, C.; Caminero-Huertas, S.; Romero, A.; Valverde, J.L.; Sánchez-Silva, L. Effects of freeze-drying conditions on aerogel properties. J. Mater. Sci. 2016, 51, 8977–8985. [CrossRef] Yang, J.; Xia, Y.; Xu, P.; Chen, B. Super-elastic and highly hydrophobic/superoleophilic sodium alginate/cellulose aerogel for oil/water separation. Cellulose 2018, 25, 3533–3544. [CrossRef] Zheng, T.; Li, A.; Li, Z.; Hu, W.; Shao, L.; Lu, L.; Cao, Y.; Chen, Y. Mechanical reinforcement of a cellulose aerogel with nanocrystalline cellulose as reinforcer. RSC Adv. 2017, 7, 34461–34465. [CrossRef] Qin, L.; Zhao, X.; He, Y.; Wang, H.; Wei, H.; Zhu, Q.; Zhang, T.; Qin, Y.; Du, A. Preparation, characterization, and in vitro evaluation of resveratrol-loaded cellulose aerogel. Materials 2020, 13, 1624. [CrossRef]
Antibiotics 2020, 9, 648
60. 61. 62.
63. 64. 65.
66. 67. 68. 69. 70. 71. 72. 73.
20 of 25
Raman, S.; Keil, C.; Dieringer, P.; Hübner, C.; Bueno, A.; Gurikov, P.; Nissen, J.; Holtkamp, M.; Karst, U.; Haase, H. Alginate aerogels carrying calcium, zinc and silver cations for wound care: Fabrication and metal detection. J. Supercrit. Fluids 2019, 153, 104545. [CrossRef] Nawaz, M.; Moztahida, M.; Kim, J.; Shahzad, A.; Jang, J.; Miran, W.; Lee, D.S. Photodegradation of microcystin-LR using graphene-TiO2 /sodium alginate aerogels. Carbohydr. Polym. 2018, 199, 109–118. [CrossRef] [PubMed] Baldino, L.; Cardea, S.; Scognamiglio, M.; Reverchon, E. A new tool to produce alginate-based aerogels for medical applications, by supercritical gel drying. J. Supercrit. Fluids 2019, 146, 152–158. [CrossRef] Li, Y.; Zhang, H.; Fan, M.; Zheng, P.; Zhuang, J.; Chen, L. A robust salt-tolerant superoleophobic alginate/graphene oxide aerogel for efficient oil/water separation in marine environments. Sci. Rep. 2017, 7, 46379. [CrossRef] [PubMed] Mallepally, R.R.; Bernard, I.; Marin, M.A.; Ward, K.R.; McHugh, M.A. Superabsorbent alginate aerogels. J. Supercrit. Fluids 2013, 79, 202–208. [CrossRef] De Cicco, F.; Russo, P.; Reverchon, E.; García-González, C.A.; Aquino, R.P.; Del Gaudio, P. Prilling and supercritical drying: A successful duo to produce core-shell polysaccharide aerogel beads for wound healing. Carbohydr. Polym. 2016, 147, 482–489. [CrossRef] Robitzer, M.; David, L.; Rochas, C.; Di Renzo, F.; Quignard, F. Nanostructure of calcium alginate aerogels obtained from multistep solvent exchange route. Langmuir 2008, 24, 12547–12552. [CrossRef] Deze, E.G.; Papageorgiou, S.K.; Favvas, E.P.; Katsaros, F.K. Porous alginate aerogel beads for effective and rapid heavy metal sorption from aqueous solutions: Effect of porosity in Cu2+ and Cd2+ ion sorption. Chem. Eng. J. 2012, 209, 537–546. [CrossRef] Franco, P.; Pessolano, E.; Belvedere, R.; Petrella, A.; De Marco, I. Supercritical impregnation of mesoglycan into calcium alginate aerogel for wound healing. J. Supercrit. Fluids 2020, 157, 104711. [CrossRef] Chen, K.; Zhang, H. Alginate/pectin aerogel microspheres for controlled release of proanthocyanidins. Int. J. Biol. Macromol. 2019, 136, 936–943. [CrossRef] Neši´c, A.; Gordi´c, M.; Davidovi´c, S.; Radovanovi´c, Ž.; Nedeljkovi´c, J.; Smirnova, I.; Gurikov, P. Pectin-based nanocomposite aerogels for potential insulated food packaging application. Carbohydr. Polym. 2018, 195, 128–135. [CrossRef] Zhu, F. Starch based aerogels: Production, properties and applications. Trends Food Sci. Technol. 2019, 89, 1–10. [CrossRef] Obaidat, R.M.; Alnaief, M.; Mashaqbeh, H. Investigation of carrageenan aerogel microparticles as a potential drug carrier. Aaps Pharmscitech 2018, 19, 2226–2236. [CrossRef] [PubMed] Zhang, W.; Shi, S.; Zhu, W.; Huang, L.; Yang, C.; Li, S.; Liu, X.; Wang, R.; Hu, N.; Suo, Y. Agar aerogel containing small-sized zeolitic imidazolate framework loaded carbon nitride: A solar-triggered regenerable decontaminant for convenient and enhanced water purification. ACS Sustain. Chem. Eng. 2017, 5, 9347–9354. [CrossRef] Bilanovic, D.; Starosvetsky, J.; Armon, R.H. Preparation of biodegradable xanthan–glycerol hydrogel, foam, film, aerogel and xerogel at room temperature. Carbohydr. Polym. 2016, 148, 243–250. [CrossRef] [PubMed] Dogenski, M.; Navarro-Díaz, H.J.; de Oliveira, J.V.; Ferreira, S.R.S. Properties of starch-based aerogels incorporated with agar or microcrystalline cellulose. Food Hydrocoll. 2020, 108, 106033. [CrossRef] Baudron, V.; Taboada, M.; Gurikov, P.; Smirnova, I.; Whitehouse, S. Production of starch aerogel in form of monoliths and microparticles. Colloid Polym. Sci. 2020, 298, 477–494. [CrossRef] Chen, L.; Li, Y.; Du, Q.; Wang, Z.; Xia, Y.; Yedinak, E.; Lou, J.; Ci, L. High performance agar/graphene oxide composite aerogel for methylene blue removal. Carbohydr. Polym. 2017, 155, 345–353. [CrossRef] Ulker, Z.; Erkey, C. An emerging platform for drug delivery: Aerogel based systems. J. Control. Release 2014, 177, 51–63. [CrossRef] ˇ c, M.; Tomi´c, S.; Beki´c, M. Immunological aspects of nanocellulose. Immunol. Lett. 2020, 222, 80–89. Coli´ [CrossRef] Edwards, J.V.; Fontenot, K.R.; Prevost, N.T.; Pircher, N.; Liebner, F.; Condon, B.D. Preparation, characterization and activity of a peptide-cellulosic aerogel protease sensor from cotton. Sensors 2016, 16, 1789. [CrossRef] Edwards, J.V.; Fontenot, K.; Liebner, F.; French, A.D.; Condon, B.D. Structure/function analysis of cotton-based peptide-cellulose conjugates: Spatiotemporal/kinetic assessment of protease aerogels compared to nanocrystalline and paper cellulose. Int. J. Mol. Sci. 2018, 19, 840. [CrossRef] [PubMed]
Antibiotics 2020, 9, 648
86. 87. 88. 89. 90. 91.
21 of 25
Li, Y.; Zhao, M.; Chen, J.; Fan, S.; Liang, J.; Ding, L.; Chen, S. Flexible chitosan/carbon nanotubes aerogel, a robust matrix for in-situ growth and non-enzymatic biosensing applications. Sens. Actuators B Chem. 2016, 232, 750–757. [CrossRef] Fontenot, K.; Edwards, J.; Pircher, N.; Liebner, F.; Prevost, N. Peptide Derivatized Cellulosic Aerogel from Cotton As a Point of Care Diagnostic Protease Sensor; Amer Chemical Soc: Washington, DC, USA, 2016. Muñoz-Ruíz, A.; Escobar-García, D.M.; Quintana, M.; Pozos-Guillén, A.; Flores, H. Synthesis and characterization of a new collagen-alginate aerogel for tissue engineering. J. Nanomater. 2019, 2019, 2875375. Osorio, D.A.; Lee, B.E.; Kwiecien, J.M.; Wang, X.; Shahid, I.; Hurley, A.L.; Cranston, E.D.; Grandfield, K. Cross-linked cellulose nanocrystal aerogels as viable bone tissue scaffolds. Acta Biomater. 2019, 87, 152–165. [CrossRef] [PubMed] Quraishi, S.; Martins, M.; Barros, A.A.; Gurikov, P.; Raman, S.; Smirnova, I.; Duarte, A.R.C.; Reis, R.L. Novel non-cytotoxic alginate–lignin hybrid aerogels as scaffolds for tissue engineering. J. Supercrit. Fluids 2015, 105, 1–8. [CrossRef] Kumari, R.; Dutta, P. Physicochemical and biological activity study of genipin-crosslinked chitosan scaffolds prepared by using supercritical carbon dioxide for tissue engineering applications. Int. J. Biol. Macromol. 2010, 46, 261–266. [CrossRef] Zhao, J.; Lu, C.; He, X.; Zhang, X.; Zhang, W.; Zhang, X. Polyethylenimine-grafted cellulose nanofibril aerogels as versatile vehicles for drug delivery. ACS Appl. Mater. Interfaces 2015, 7, 2607–2615. [CrossRef] Gonçalves, V.S.; Gurikov, P.; Poejo, J.; Matias, A.A.; Heinrich, S.; Duarte, C.M.; Smirnova, I. Alginate-based hybrid aerogel microparticles for mucosal drug delivery. Eur. J. Pharm. Biopharm. 2016, 107, 160–170. [CrossRef] Mohammadian, M.; Kashi, T.S.J.; Erfan, M.; Soorbaghi, F.P. In-vitro study of Ketoprofen release from synthesized silica aerogels (as drug carriers) and evaluation of mathematical kinetic release models. Iran. J. Pharm. Res. IJPR 2018, 17, 818. Qin, L.; He, Y.; Zhao, X.; Zhang, T.; Qin, Y.; Du, A. Preparation, characterization, and in vitro sustained release profile of resveratrol-loaded silica aerogel. Molecules 2020, 25, 2752. [CrossRef] Wang, L.; Mu, R.-J.; Lin, L.; Chen, X.; Lin, S.; Ye, Q.; Pang, J. Bioinspired aerogel based on konjac glucomannan and functionalized carbon nanotube for controlled drug release. Int. J. Biol. Macromol. 2019, 133, 693–701. [CrossRef] [PubMed] Esquivel-Castro, T.A.; Ibarra-Alonso, M.; Oliva, J.; Martínez-Luévanos, A. Porous aerogel and core/shell nanoparticles for controlled drug delivery: A review. Mater. Sci. Eng. C 2019, 96, 915–940. [CrossRef] [PubMed] Zhang, F.; Wu, W.; Zhang, X.; Meng, X.; Tong, G.; Deng, Y. Temperature-sensitive poly-NIPAm modified cellulose nanofibril cryogel microspheres for controlled drug release. Cellulose 2016, 23, 415–425. [CrossRef] Lovskaya, D.; Lebedev, A.; Menshutina, N. Aerogels as drug delivery systems: In vitro and in vivo evaluations. J. Supercrit. Fluids 2015, 106, 115–121. [CrossRef] Feng, J.; Nguyen, S.T.; Fan, Z.; Duong, H.M. Advanced fabrication and oil absorption properties of super-hydrophobic recycled cellulose aerogels. Chem. Eng. J. 2015, 270, 168–175. [CrossRef] Zhang, Z.; Wang, X.; Gao, M.; Zhao, Y.; Chen, Y. Sustained release of an essential oil by a hybrid cellulose nanofiber foam system. Cellulose 2020, 27, 2709–2721. [CrossRef] Han, W.; Han, D.W.; Chan, C.K.; Li, Y.; Chang, Q.; Yeung, K.L. silica alcogel containing essential oil for air and surface disinfections. Am. Chem. Soc. 2013, 245, 7–11. Uddin, K.M.; Orelma, H.; Mohammadi, P.; Borghei, M.; Laine, J.; Linder, M.; Rojas, O.J. Retention of lysozyme activity by physical immobilization in nanocellulose aerogels and antibacterial effects. Cellulose 2017, 24, 2837–2848. [CrossRef] Wang, P.; Zhao, J.; Xuan, R.; Wang, Y.; Zou, C.; Zhang, Z.; Wan, Y.; Xu, Y. Flexible and monolithic zinc oxide bionanocomposite foams by a bacterial cellulose mediated approach for antibacterial applications. Dalton Trans. 2014, 43, 6762–6768. [CrossRef] Luong, N.D.; Lee, Y.; Nam, J.-D. Highly-loaded silver nanoparticles in ultrafine cellulose acetate nanofibrillar aerogel. Eur. Polym. J. 2008, 44, 3116–3121. [CrossRef] Zhang, S.; Wu, D.; Wan, L.; Tan, H.; Fu, R. Adsorption and antibacterial activity of silver-dispersed carbon aerogels. J. Appl. Polym. Sci. 2006, 102, 1030–1037. [CrossRef]
Antibiotics 2020, 9, 648
95. 96. 97. 98.
99. 100. 101. 102. 103. 104.
108. 109. 110. 111.
112. 113. 114.
22 of 25
Bheekhun, N.; Talib, A.; Rahim, A.; Hassan, M.R. Aerogels in aerospace: An overview. Adv. Mater. Sci. Eng. 2013, 2013, 406065. [CrossRef] Pekala, R. Organic aerogels from the polycondensation of resorcinol with formaldehyde. J. Mater. Sci. 1989, 24, 3221–3227. [CrossRef] Leventis, N.; Sotiriou-Leventis, C.; Zhang, G.; Rawashdeh, A.-M.M. Nanoengineering strong silica aerogels. Nano Lett. 2002, 2, 957–960. [CrossRef] Xiong, R.; Lu, C.; Wang, Y.; Zhou, Z.; Zhang, X. Nanofibrillated cellulose as the support and reductant for the facile synthesis of Fe3O4/Ag nanocomposites with catalytic and antibacterial activity. J. Mater. Chem. A 2013, 1, 14910–14918. [CrossRef] Zhou, B.; Li, Y.; Deng, H.; Hu, Y.; Li, B. Antibacterial multilayer films fabricated by layer-by-layer immobilizing lysozyme and gold nanoparticles on nanofibers. Colloids Surf. B Biointerfaces 2014, 116, 432–438. [CrossRef] Korehei, R.; Kadla, J.F. Encapsulation of T4 bacteriophage in electrospun poly (ethylene oxide)/cellulose diacetate fibers. Carbohydr. Polym. 2014, 100, 150–157. [CrossRef] Liu, K.; Chen, L.; Huang, L.; Ni, Y.; Sun, B. Enhancing antibacterium and strength of cellulosic paper by coating triclosan-loaded nanofibrillated cellulose (NFC). Carbohydr. Polym. 2015, 117, 996–1001. [CrossRef] Henschen, J.; Illergård, J.; Larsson, P.A.; Ek, M.; Wågberg, L. Contact-active antibacterial aerogels from cellulose nanofibrils. Colloids Surf. B Biointerfaces 2016, 146, 415–422. [CrossRef] Ye, S.; He, S.; Su, C.; Jiang, L.; Wen, Y.; Zhu, Z.; Shao, W. Morphological, release and antibacterial performances of amoxicillin-loaded cellulose aerogels. Molecules 2018, 23, 2082. [CrossRef] Xiao, Y.; Rong, L.; Wang, B.; Mao, Z.; Xu, H.; Zhong, Y.; Zhang, L.; Sui, X. A light-weight and high-efficacy antibacterial nanocellulose-based sponge via covalent immobilization of gentamicin. Carbohydr. Polym. 2018, 200, 595–601. [CrossRef] [PubMed] López-Iglesias, C.; Barros, J.; Ardao, I.; Monteiro, F.J.; Alvarez-Lorenzo, C.; Gómez-Amoza, J.L.; García-González, C.A. Vancomycin-loaded chitosan aerogel particles for chronic wound applications. Carbohydr. Polym. 2019, 204, 223–231. [CrossRef] [PubMed] Zhang, S.; Li, L.; Ren, X.; Huang, T.-S. N-halamine modified multiporous bacterial cellulose with enhanced antibacterial and hemostatic properties. Int. J. Biol. Macromol. 2020, 161, 1070–1078. [CrossRef] [PubMed] Sahariah, P.; Snorradóttir, B.S.; Hjálmarsdóttir, M.Á.; Sigurjónsson, Ó.E.; Másson, M. Experimental design for determining quantitative structure activity relationship for antibacterial chitosan derivatives. J. Mater. Chem. B 2016, 4, 4762–4770. [CrossRef] Raafat, D.; Von Bargen, K.; Haas, A.; Sahl, H.-G. Insights into the mode of action of chitosan as an antibacterial compound. Appl. Environ. Microbiol. 2008, 74, 3764–3773. [CrossRef] Goy, R.C.; Britto, D.d.; Assis, O.B. A review of the antimicrobial activity of chitosan. Polímeros 2009, 19, 241–247. [CrossRef] Wu, J.; Su, C.; Jiang, L.; Ye, S.; Liu, X.; Shao, W. Green and facile preparation of chitosan sponges as potential wound dressings. ACS Sustain. Chem. Eng. 2018, 6, 9145–9152. [CrossRef] López-Iglesias, C.; Barros, J.; Ardao, I.; Gurikov, P.; Monteiro, F.J.; Smirnova, I.; Alvarez-Lorenzo, C.; García-González, C.A. Jet cutting technique for the production of chitosan aerogel microparticles loaded with vancomycin. Polymers 2020, 12, 273. [CrossRef] Yang, H.; Zhang, S.; Yan, J. Chitosan-Reinforced MFC/NFC Aerogel and Antibacterial Property. Adv. Polym. Technol. 2020, 2020, 7890215. [CrossRef] Wan, C.; Jiao, Y.; Sun, Q.; Li, J. Preparation, characterization, and antibacterial properties of silver nanoparticles embedded into cellulose aerogels. Polym. Compos. 2016, 37, 1137–1142. [CrossRef] Wasim, M.; Khan, M.R.; Mushtaq, M.; Naeem, A.; Han, M.; Wei, Q. Surface modification of bacterial cellulose by copper and zinc oxide sputter coating for uv-resistance/antistatic/antibacterial characteristics. Coatings 2020, 10, 364. [CrossRef] Li, S.; Hao, X.; Dai, X.; Tao, T. Rapid Photocatalytic Degradation of pollutant from water under UV and sunlight via cellulose nanofiber aerogel wrapped by TiO2. J. Nanomater. 2018, 2018, 8752015. [CrossRef] Darpentigny, C.; Marcoux, P.R.; Menneteau, M.; Michel, B.; Ricoul, F.; Jean, B.; Bras, J.; Nonglaton, G. Antimicrobial cellulose nanofibril porous materials obtained by supercritical impregnation of thymol. ACS Appl. Bio Mater. 2020, 3, 2965–2975. [CrossRef]
Antibiotics 2020, 9, 648
23 of 25
117. Yahya, E.B.; Alhawari, S.M.; Amhimmid, K.; AbuAeshah, R.H.A.; Saada, A.O. Evaluation of in-vitroantibacterial activity of aqueous and alcoholic extracts of the peels punica granatum and olea europaea leaves. J. Sci. Technol. 2018, 2, 36–40. 118. Navarro, J.R.; Rostami, J.; Ahlinder, A.; Mietner, J.B.; Bernin, D.; Saake, B.; Edlund, U. Surface-initiated controlled radical polymerization approach to in situ cross-link cellulose nanofibrils with inorganic nanoparticles. Biomacromolecules 2020, 21, 1952–1961. [CrossRef] [PubMed] 119. Shen, Z.; Han, G.; Wang, X.; Luo, J.; Sun, R. An ultra-light antibacterial bagasse–AgNP aerogel. J. Mater. Chem. B 2017, 5, 1155–1158. [CrossRef] 120. Salomoni, R.; Léo, P.; Montemor, A.; Rinaldi, B.; Rodrigues, M. Antibacterial effect of silver nanoparticles in Pseudomonas aeruginosa. Nanotechnol. Sci. Appl. 2017, 10, 115. [CrossRef] 121. Tang, S.; Zheng, J. Antibacterial activity of silver nanoparticles: Structural effects. Adv. Healthc. Mater. 2018, 7, 1701503. [CrossRef] 122. Vijaya, J.J.; Jayaprakash, N.; Kombaiah, K.; Kaviyarasu, K.; Kennedy, L.J.; Ramalingam, R.J.; Al-Lohedan, H.A.; Mansoor-Ali, V.; Maaza, M. Bioreduction potentials of dried root of Zingiber officinale for a simple green synthesis of silver nanoparticles: Antibacterial studies. J. Photochem. Photobiol. B Biol. 2017, 177, 62–68. [CrossRef] 123. Cvjetko, P.; Miloši´c, A.; Domijan, A.-M.; Vrˇcek, I.V.; Toli´c, S.; Štefani´c, P.P.; Letofsky-Papst, I.; Tkalec, M.; Balen, B. Toxicity of silver ions and differently coated silver nanoparticles in Allium cepa roots. Ecotoxicol. Environ. Saf. 2017, 137, 18–28. [CrossRef] 124. Tarrés, Q.; Oliver-Ortega, H.; Alcalà, M.; Espinach, F.X.; Mutjé, P.; Delgado-Aguilar, M. Research on the Strengthening Advantages on Using Cellulose Nanofibers as Polyvinyl Alcohol Reinforcement. Polymers 2020, 12, 974. [CrossRef] [PubMed] 125. Tayeb, A.H.; Amini, E.; Ghasemi, S.; Tajvidi, M. Cellulose nanomaterials—Binding properties and applications: A review. Molecules 2018, 23, 2684. [CrossRef] [PubMed] 126. Frka-Petesic, B.; Guidetti, G.; Kamita, G.; Vignolini, S. Controlling the photonic properties of cholesteric cellulose nanocrystal films with magnets. Adv. Mater. 2017, 29, 1701469. [CrossRef] [PubMed] 127. Wei, D.W.; Wei, H.; Gauthier, A.C.; Song, J.; Jin, Y.; Xiao, H. Superhydrophobic modification of cellulose and cotton textiles: Methodologies and applications. J. Bioresour. Bioprod. 2020, 5, 1–15. [CrossRef] 128. Kumari, P.; Pathak, G.; Gupta, R.; Sharma, D.; Meena, A. Cellulose nanofibers from lignocellulosic biomass of lemongrass using enzymatic hydrolysis: Characterization and cytotoxicity assessment. DARU J. Pharm. Sci. 2019, 27, 683–693. [CrossRef] 129. Lee, I.; Kim, S.-H.; Rethinasabapathy, M.; Haldorai, Y.; Lee, G.-W.; Choe, S.R.; Jang, S.-C.; Kang, S.-M.; Han, Y.-K.; Roh, C. Porous 3D Prussian blue/cellulose aerogel as a decorporation agent for removal of ingested cesium from the gastrointestinal tract. Sci. Rep. 2018, 8, 1–14. [CrossRef] 130. Souza, S.F.; Mariano, M.; Reis, D.; Lombello, C.B.; Ferreira, M.; Sain, M. Cell interactions and cytotoxic studies of cellulose nanofibers from Curauá natural fibers. Carbohydr. Polym. 2018, 201, 87–95. [CrossRef] 131. Nordli, H.R.; Chinga-Carrasco, G.; Rokstad, A.M.; Pukstad, B. Producing ultrapure wood cellulose nanofibrils and evaluating the cytotoxicity using human skin cells. Carbohydr. Polym. 2016, 150, 65–73. [CrossRef] 132. Batista, M.; Gonçalves, V.S.; Gaspar, F.; Nogueira, I.; Matias, A.A.; Gurikov, P. Novel alginate-chitosan aerogel fibres for potential wound healing applications. Int. J. Biol. Macromol. 2020, 156, 773–782. [CrossRef] 133. Martins, M.; Barros, A.A.; Quraishi, S.; Gurikov, P.; Raman, S.; Smirnova, I.; Duarte, A.R.C.; Reis, R.L. Preparation of macroporous alginate-based aerogels for biomedical applications. J. Supercrit. Fluids 2015, 106, 152–159. [CrossRef] 134. Trucillo, P.; Cardea, S.; Baldino, L.; Reverchon, E. Production of liposomes loaded alginate aerogels using two supercritical CO2 assisted techniques. J. CO2 Util. 2020, 39, 101161. [CrossRef] 135. Ma, R.; Wang, Y.; Qi, H.; Shi, C.; Wei, G.; Xiao, L.; Huang, Z.; Liu, S.; Yu, H.; Teng, C. Nanocomposite sponges of sodium alginate/graphene oxide/polyvinyl alcohol as potential wound dressing: In vitro and in vivo evaluation. Compos. Part B Eng. 2019, 167, 396–405. [CrossRef] 136. Abdelgawad, A.M.; El-Naggar, M.E.; Elsherbiny, D.A.; Ali, S.; Abdel-Aziz, M.S.; Abdel-Monem, Y.K. Antibacterial carrageenan/cellulose nanocrystal system loaded with silver nanoparticles, prepared via solid-state technique. J. Environ. Chem. Eng. 2020, 8, 104276. [CrossRef]
Antibiotics 2020, 9, 648
24 of 25
137. Nisar, T.; Wang, Z.-C.; Yang, X.; Tian, Y.; Iqbal, M.; Guo, Y. Characterization of citrus pectin films integrated with clove bud essential oil: Physical, thermal, barrier, antioxidant and antibacterial properties. Int. J. Biol. Macromol. 2018, 106, 670–680. [CrossRef] [PubMed] 138. Liang, Y.; Chen, B.; Li, M.; He, J.; Yin, Z.; Guo, B. Injectable antimicrobial conductive hydrogels for wound disinfection and infectious wound healing. Biomacromolecules 2020, 21, 1841–1852. [CrossRef] [PubMed] 139. Sen, C.K.; Gordillo, G.M.; Roy, S.; Kirsner, R.; Lambert, L.; Hunt, T.K.; Gottrup, F.; Gurtner, G.C.; Longaker, M.T. Human skin wounds: A major and snowballing threat to public health and the economy. Wound Repair Regen. 2009, 17, 763–771. [CrossRef] [PubMed] 140. Sen, C.K. Human wounds and its burden: An updated compendium of estimates. Adv. Wound Care 2019. [CrossRef] 141. Aderibigbe, B.A.; Buyana, B. Alginate in wound dressings. Pharmaceutics 2018, 10, 42. [CrossRef] 142. Schreml, S.; Meier, R.J.; Kirschbaum, M.; Kong, S.C.; Gehmert, S.; Felthaus, O.; Küchler, S.; Sharpe, J.R.; Wöltje, K.; Weiß, K.T. Luminescent dual sensors reveal extracellular pH-gradients and hypoxia on chronic wounds that disrupt epidermal repair. Theranostics 2014, 4, 721. [CrossRef] 143. Kur-Piotrowska, A.; Bukowska, J.; Kopcewicz, M.M.; Dietrich, M.; Nynca, J.; Slowinska, M.; Gawronska-Kozak, B. Foxn1 expression in keratinocytes is stimulated by hypoxia: Further evidence of its role in skin wound healing. Sci. Rep. 2018, 8, 1–14. [CrossRef] 144. Koehler, J.; Brandl, F.P.; Goepferich, A.M. Hydrogel wound dressings for bioactive treatment of acute and chronic wounds. Eur. Polym. J. 2018, 100, 1–11. [CrossRef] 145. He, H.; Xia, D.L.; Chen, Y.P.; Li, X.D.; Chen, C.; Wang, Y.F.; Shen, L.; Hu, Y.L.; Gu, H.Y. Evaluation of a two-stage antibacterial hydrogel dressing for healing in an infected diabetic wound. J. Biomed. Mater. Res. Part B Appl. Biomater. 2017, 105, 1808–1817. [CrossRef] [PubMed] 146. Jia, J.; Wang, C. A facile restructuring of 3D high water absorption aerogels from methoxy polyethylene glycol-polycaprolactone (mPEG-PCL) nanofibers. Mater. Sci. Eng. C 2019, 94, 965–975. [CrossRef] 147. Sreekumar, P.; Thomas, S.P.; marc Saiter, J.; Joseph, K.; Unnikrishnan, G.; Thomas, S. Effect of fiber surface modification on the mechanical and water absorption characteristics of sisal/polyester composites fabricated by resin transfer molding. Compos. Part A Appl. Sci. Manuf. 2009, 40, 1777–1784. [CrossRef] 148. Zhao, X.; Wu, H.; Guo, B.; Dong, R.; Qiu, Y.; Ma, P.X. Antibacterial anti-oxidant electroactive injectable hydrogel as self-healing wound dressing with hemostasis and adhesiveness for cutaneous wound healing. Biomaterials 2017, 122, 34–47. [CrossRef] 149. Ko, E.; Kim, H. Preparation of chitosan aerogel crosslinked in chemical and ionical ways by non-acid condition for wound dressing. Int. J. Biol. Macromol. 2020, 164, 2177–2185. [CrossRef] 150. Lu, H.; Yuan, L.; Yu, X.; Wu, C.; He, D.; Deng, J. Recent advances of on-demand dissolution of hydrogel dressings. Burn. Trauma 2018, 6, 35. [CrossRef] 151. Deuber, F.; Adlhart, C. Tailoring the microstructure of ultra-light nanofiber aerogels by solid templating and their application as wound dressing materials. À Jour SVC Chem. Life Sci. Biotechnol. 2018, 18, 17–19. 152. Martinez, P.R.; Goyanes, A.; Basit, A.W.; Gaisford, S. Fabrication of drug-loaded hydrogels with stereolithographic 3D printing. Int. J. Pharm. 2017, 532, 313–317. [CrossRef] 153. Uzun, M. Developments in nonwovens for wound dressings. In Advances in Technical Nonwovens; Elsevier: Amsterdam, The Netherlands, 2016; pp. 443–472. 154. Gould, L.J.; Abadir, P.M.; White-Chu, E.F. Age, frailty, and impaired wound healing. Princ. Pract. Geriatr. Surg. 2020, 2020, 465–482. 155. Simões, D.; Miguel, S.P.; Ribeiro, M.P.; Coutinho, P.; Mendonça, A.G.; Correia, I.J. Recent advances on antimicrobial wound dressing: A review. Eur. J. Pharm. Biopharm. 2018, 127, 130–141. [CrossRef] [PubMed] 156. Hamed, I.; Özogul, F.; Regenstein, J.M. Industrial applications of crustacean by-products (chitin, chitosan, and chitooligosaccharides): A review. Trends Food Sci. Technol. 2016, 48, 40–50. [CrossRef] 157. Fan, X.; Li, Y.; Li, X.; Wu, Y.; Tang, K.; Liu, J.; Zheng, X.; Wan, G. Injectable antibacterial cellulose nanofiber/chitosan aerogel with rapid shape recovery for noncompressible hemorrhage. Int. J. Biol. Macromol. 2020, 154, 1185–1193. [CrossRef] [PubMed] 158. Thomas, S.; Uzun, M. Testing dressings and wound management materials. In Advanced Textiles for Wound Care; Elsevier: Amsterdam, The Netherlands, 2019; pp. 23–54. 159. Suarato, G.; Bertorelli, R.; Athanassiou, A. Borrowing from Nature: Biopolymers and biocomposites as smart wound care materials. Front. Bioeng. Biotechnol. 2018, 6, 137. [CrossRef] [PubMed]
Antibiotics 2020, 9, 648
25 of 25
160. Jiang, T.; James, R.; Kumbar, S.G.; Laurencin, C.T. Chitosan as a biomaterial: Structure, properties, and applications in tissue engineering and drug delivery. In Natural and Synthetic Biomedical Polymers; Elsevier: Amsterdam, The Netherlands, 2014; pp. 91–113. 161. Teixeira, B.; Marques, A.; Ramos, C.; Neng, N.R.; Nogueira, J.M.; Saraiva, J.A.; Nunes, M.L. Chemical composition and antibacterial and antioxidant properties of commercial essential oils. Ind. Crop. Prod. 2013, 43, 587–595. [CrossRef] 162. Biranje, S.S.; Madiwale, P.V.; Patankar, K.C.; Chhabra, R.; Bangde, P.; Dandekar, P.; Adivarekar, R.V. Cytotoxicity and hemostatic activity of chitosan/carrageenan composite wound healing dressing for traumatic hemorrhage. Carbohydr. Polym. 2020, 239, 116106. [CrossRef] 163. Choudhary, P.; Ramalingam, B.; Das, S.K. Fabrication of Chitosan Reinforced Multifunctional Graphene Nanocomposite as Antibacterial Scaffolds for Hemorrhage Control and wound Healing Application. ACS Biomater. Sci. Eng. 2020. [CrossRef] 164. Fan, X.; Li, Y.; Li, N.; Wan, G.; Ali, M.A.; Tang, K. Rapid hemostatic chitosan/cellulose composite sponge by alkali/urea method for massive haemorrhage. Int. J. Biol. Macromol. 2020, 146, 2769–2778. [CrossRef] 165. Teixeira, M.L.; Marcussi, S.; de CS Rezende, D.A.; Magalhães, M.L.; Nelson, D.L.; das G Cardoso, M. Essential oil from lippia origanoides (verbenaceae): Haemostasis and enzymes activity alterations. Med. Chem. 2019, 15, 207–214. [CrossRef] 166. Moghimi, R.; Aliahmadi, A.; Rafati, H. Antibacterial hydroxypropyl methyl cellulose edible films containing nanoemulsions of Thymus daenensis essential oil for food packaging. Carbohydr. Polym. 2017, 175, 241–248. [CrossRef] 167. Pereira, S.G.; Moura, J.; Carvalho, E.; Empadinhas, N. Microbiota of chronic diabetic wounds: Ecology, impact, and potential for innovative treatment strategies. Front. Microbiol. 2017, 8, 1791. [CrossRef] [PubMed] 168. Wang, C.; Wang, M.; Xu, T.; Zhang, X.; Lin, C.; Gao, W.; Xu, H.; Lei, B.; Mao, C. Engineering bioactive self-healing antibacterial exosomes hydrogel for promoting chronic diabetic wound healing and complete skin regeneration. Theranostics 2019, 9, 65. [CrossRef] [PubMed] 169. Camarero-Espinosa, S.; Endes, C.; Mueller, S.; Petri-Fink, A.; Rothen-Rutishauser, B.; Weder, C.; Clift, M.J.D.; Foster, E.J. Elucidating the potential biological impact of cellulose nanocrystals. Fibers 2016, 4, 21. [CrossRef] 170. Seabra, A.B.; Bernardes, J.S.; Fávaro, W.J.; Paula, A.J.; Durán, N. Cellulose nanocrystals as carriers in medicine and their toxicities: A review. Carbohydr. Polym. 2018, 181, 514–527. [CrossRef] 171. Endes, C.; Camarero-Espinosa, S.; Mueller, S.; Foster, E.; Petri-Fink, A.; Rothen-Rutishauser, B.; Weder, C.; Clift, M. A critical review of the current knowledge regarding the biological impact of nanocellulose. J. Nanobiotechnology 2016, 14, 78. [CrossRef] 172. Yahya, E.B.; Alfallous, K.A.; Wali, A.; Hameid, S.; Zwaid, H. Growth Rate and Antibiotic Sensitivity Effect of Some Natural and Petroleum Based Materials on Staphylococcus aureus. Int. J. Res. Appl. Sci. Biotechnol. 2020, 7, 7–11. 173. Pan, X.; Redding, J.E.; Wiley, P.A.; Wen, L.; McConnell, J.S.; Zhang, B. Mutagenicity evaluation of metal oxide nanoparticles by the bacterial reverse mutation assay. Chemosphere 2010, 79, 113–116. [CrossRef] © 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).